# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2018

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1828904'
_audit_update_record             
;
2018-03-13 deposited with the CCDC.
2018-05-31 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C74 H156 La2 N2 O46 Ti6'
_chemical_formula_weight         2375.03

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ti Ti 0.2776 0.4457 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.6585(5)
_cell_length_b                   21.7777(10)
_cell_length_c                   24.1796(12)
_cell_angle_alpha                106.086(4)
_cell_angle_beta                 90.174(4)
_cell_angle_gamma                94.037(4)
_cell_volume                     5882.5(5)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    12431
_cell_measurement_theta_min      3.0
_cell_measurement_theta_max      26.3

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    1.332
_exptl_crystal_F_000             2424
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.500
_exptl_crystal_size_mid          0.450
_exptl_crystal_size_min          0.200
_exptl_absorpt_coefficient_mu    1.171
_shelx_estimated_absorpt_T_min   0.592
_shelx_estimated_absorpt_T_max   0.800
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.84844
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Xcalibur, Atlas, Gemini'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            66241
_diffrn_reflns_av_unetI/netI     0.0859
_diffrn_reflns_av_R_equivalents  0.0643
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_theta_min         2.901
_diffrn_reflns_theta_max         25.200
_diffrn_reflns_theta_full        25.200
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_point_group_measured_fraction_full 0.998
_reflns_number_total             21132
_reflns_number_gt                12980
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0806P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         21132
_refine_ls_number_parameters     1156
_refine_ls_number_restraints     71
_refine_ls_R_factor_all          0.1078
_refine_ls_R_factor_gt           0.0560
_refine_ls_wR_factor_ref         0.1661
_refine_ls_wR_factor_gt          0.1440
_refine_ls_goodness_of_fit_ref   1.027
_refine_ls_restrained_S_all      1.036
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
La1 La -0.03359(3) 0.46041(2) 0.40276(2) 0.03757(11) Uani 1 1 d . . . . .
La2 La 0.47905(3) 0.53700(2) 0.09698(2) 0.03957(12) Uani 1 1 d . . . . .
Ti1 Ti 0.01176(9) 0.24639(5) 0.50125(4) 0.0468(3) Uani 1 1 d . . . . .
Ti2 Ti 0.17924(10) 0.17790(6) 0.40926(5) 0.0608(3) Uani 1 1 d . . . . .
Ti3 Ti -0.05191(10) 0.17320(6) 0.34197(5) 0.0573(3) Uani 1 1 d . . . . .
Ti4 Ti 0.53519(12) 0.82435(6) 0.16358(5) 0.0695(4) Uani 1 1 d . . . . .
Ti5 Ti 0.75792(11) 0.82407(7) 0.09167(6) 0.0687(4) Uani 1 1 d . . . . .
Ti6 Ti 0.43277(10) 0.24402(6) -0.00240(5) 0.0541(3) Uani 1 1 d . . . . .
O1 O -0.1516(4) 0.1151(2) 0.3596(2) 0.0712(14) Uani 1 1 d . . . . .
O2 O 0.3014(4) 0.2059(3) 0.3781(2) 0.0874(16) Uani 1 1 d . . . . .
O3 O 0.0209(4) 0.1897(2) 0.54191(19) 0.0690(13) Uani 1 1 d . . . . .
O4 O -0.1379(3) 0.2552(2) 0.50745(17) 0.0580(12) Uani 1 1 d . . . . .
O5 O 0.1884(3) 0.2440(2) 0.48385(18) 0.0617(12) Uani 1 1 d . . . . .
O6 O 0.0198(3) 0.19774(19) 0.42290(16) 0.0520(11) Uani 1 1 d . . . . .
O7 O 0.0970(4) 0.1320(2) 0.33375(18) 0.0665(13) Uani 1 1 d . . . . .
O8 O -0.0927(4) 0.1588(2) 0.26841(19) 0.0778(15) Uani 1 1 d . . . . .
O9 O 0.0613(3) 0.2554(2) 0.33692(18) 0.0573(12) Uani 1 1 d . . . . .
O10 O -0.1536(3) 0.2496(2) 0.36847(17) 0.0528(11) Uani 1 1 d . . . . .
O11 O 0.0636(3) 0.3622(2) 0.35359(17) 0.0508(11) Uani 1 1 d . . . . .
O12 O -0.1580(3) 0.3563(2) 0.38489(17) 0.0505(10) Uani 1 1 d . . . . .
O13 O -0.1117(3) 0.4516(2) 0.30302(16) 0.0573(11) Uani 1 1 d . . . . .
O14 O -0.2258(3) 0.4873(2) 0.45072(17) 0.0595(12) Uani 1 1 d . . . . .
O15 O -0.0540(4) 0.5692(2) 0.38989(15) 0.0531(11) Uani 1 1 d . . . . .
O16 O -0.0520(4) 0.6758(2) 0.42539(16) 0.0521(10) Uani 1 1 d . . . . .
O17 O -0.0209(3) 0.6676(2) 0.52978(15) 0.0476(10) Uani 1 1 d . . . . .
O18 O -0.0057(3) 0.56085(18) 0.49795(14) 0.0378(9) Uani 1 1 d . . . . .
O19 O 0.1785(3) 0.4823(3) 0.43344(18) 0.0706(15) Uani 1 1 d . . . . .
O20 O 0.8755(5) 0.7936(3) 0.1194(3) 0.0990(18) Uani 1 1 d . . . . .
O21 O 0.4140(4) 0.3211(2) 0.07187(16) 0.0577(11) Uani 1 1 d . . . . .
O22 O 0.4357(4) 0.4271(2) 0.10856(16) 0.0589(12) Uani 1 1 d . . . . .
O23 O 0.2783(3) 0.5098(2) 0.05032(17) 0.0618(13) Uani 1 1 d . . . . .
O24 O 0.6614(4) 0.5081(2) 0.15152(19) 0.0647(13) Uani 1 1 d . . . . .
O25 O 0.4046(4) 0.5444(2) 0.19679(16) 0.0587(12) Uani 1 1 d . . . . .
O26 O 0.3814(3) 0.6415(2) 0.11771(17) 0.0536(11) Uani 1 1 d . . . . .
O27 O 0.6014(3) 0.6343(2) 0.14676(17) 0.0548(11) Uani 1 1 d . . . . .
O28 O 0.6259(4) 0.7416(2) 0.16600(18) 0.0616(12) Uani 1 1 d . . . . .
O29 O 0.4131(4) 0.7483(2) 0.13738(18) 0.0622(12) Uani 1 1 d . . . . .
O30 O 0.4369(3) 0.3315(2) -0.03190(15) 0.0501(10) Uani 1 1 d . . . . .
O31 O 0.4784(3) 0.4373(2) 0.00075(14) 0.0425(9) Uani 1 1 d . . . . .
O32 O 0.5840(4) 0.2557(2) 0.00215(18) 0.0636(12) Uani 1 1 d . . . . .
O33 O 0.4175(5) 0.1857(2) 0.0374(2) 0.0831(15) Uani 1 1 d . . . . .
O34 O 0.7458(4) 0.7617(2) 0.0153(2) 0.0716(14) Uani 1 1 d . . . . .
O35 O 0.5937(4) 0.8018(2) 0.08085(17) 0.0580(12) Uani 1 1 d . . . . .
O36 O 0.6926(4) 0.8655(2) 0.16926(19) 0.0796(15) Uani 1 1 d . . . . .
O37 O 0.5068(5) 0.8370(3) 0.2380(2) 0.0950(18) Uani 1 1 d . . . . .
O38 O 0.6852(3) 0.5149(3) 0.06509(18) 0.0738(16) Uani 1 1 d . . . . .
O39 O 0.8311(4) 0.5043(4) 0.1152(3) 0.110(2) Uani 1 1 d . . . . .
O40 O 0.2815(5) 0.4488(3) 0.2310(2) 0.0907(17) Uani 1 1 d . . . . .
O41 O 0.1556(4) 0.4886(2) 0.3472(2) 0.0670(13) Uani 1 1 d . . . . .
O42 O 0.3262(4) 0.4921(4) 0.3828(2) 0.111(2) Uani 1 1 d . . . . .
O43 O 0.8075(5) 0.8944(3) 0.0746(2) 0.101(2) Uani 1 1 d . . . . .
O44 O 0.7947(4) 0.5460(3) 0.2671(2) 0.0870(16) Uani 1 1 d . . . . .
O45 O 0.2197(5) 0.1100(3) 0.4293(2) 0.0912(17) Uani 1 1 d . U . . .
O46 O 0.4490(5) 0.8820(3) 0.1517(3) 0.1004(19) Uani 1 1 d . U . . .
N1 N 0.7283(5) 0.5087(3) 0.1117(2) 0.0671(17) Uani 1 1 d . . . . .
N2 N 0.2226(5) 0.4884(3) 0.3869(3) 0.0654(16) Uani 1 1 d . . . . .
C1 C -0.0450(5) 0.6202(3) 0.4296(2) 0.0420(14) Uani 1 1 d . . . . .
C2 C -0.0220(4) 0.6152(3) 0.4917(2) 0.0372(14) Uani 1 1 d . . . . .
C3 C -0.1093(5) 0.3055(3) 0.3708(2) 0.0446(15) Uani 1 1 d . . . . .
C4 C 0.0180(5) 0.3085(3) 0.3521(2) 0.0461(15) Uani 1 1 d . . . . .
C5 C 0.1612(7) 0.5204(6) 0.0691(5) 0.123(4) Uani 1 1 d . . . . .
C6 C 0.1117(7) 0.5682(5) 0.0465(5) 0.117(4) Uani 1 1 d . . . . .
C7 C 0.1349(9) 0.5019(8) 0.1176(5) 0.167(6) Uani 1 1 d . . . . .
C8 C 0.2733(14) 0.0486(10) 0.4455(9) 0.226(7) Uani 1 1 d . U . . .
C9 C 0.446(2) 0.8424(15) 0.2870(7) 0.324(17) Uani 1 1 d . . . . .
C10 C 0.3389(19) 0.8293(18) 0.2851(10) 0.39(2) Uani 1 1 d . . . . .
C11 C 0.347(3) 0.0795(18) 0.4818(16) 0.41(2) Uiso 1 1 d . . . . .
C12 C 0.351(2) 0.0403(13) 0.3930(12) 0.320(12) Uiso 1 1 d . . . . .
C13 C 0.2301(9) 0.3375(5) 0.2304(5) 0.121(4) Uani 1 1 d . . . . .
C14 C 0.505(3) 0.849(2) 0.3366(10) 0.44(2) Uani 1 1 d . U . . .
C15 C -0.1058(10) 0.0421(5) 0.4156(5) 0.120(3) Uani 1 1 d . . . . .
C16 C -0.3156(8) 0.0697(6) 0.3974(5) 0.138(4) Uani 1 1 d . . . . .
C17 C -0.3475(6) 0.4786(6) 0.4335(5) 0.115(4) Uani 1 1 d . . . . .
C18 C -0.4075(7) 0.4288(5) 0.4577(4) 0.107(3) Uani 1 1 d . . . . .
C19 C -0.3678(7) 0.4875(6) 0.3795(4) 0.127(4) Uani 1 1 d . . . . .
C20 C -0.1167(7) 0.3950(4) 0.2522(3) 0.074(2) Uani 1 1 d . . . . .
C21 C -0.0522(8) 0.4131(5) 0.2039(3) 0.106(3) Uani 1 1 d . . . . .
C22 C -0.2426(8) 0.3738(5) 0.2363(4) 0.114(4) Uani 1 1 d . . . . .
C23 C 0.9245(14) 0.7537(9) 0.1510(7) 0.191(7) Uani 1 1 d . . . . .
C24 C 0.4317(5) 0.3774(3) 0.0686(2) 0.0470(15) Uani 1 1 d . . . . .
C25 C 0.9758(16) 0.9625(12) 0.0853(10) 0.306(11) Uani 1 1 d . U . . .
C26 C 0.4508(4) 0.3829(3) 0.0070(2) 0.0393(14) Uani 1 1 d . . . . .
C27 C 0.4749(8) 0.5827(5) 0.2966(3) 0.107(3) Uani 1 1 d . . . . .
C28 C 0.5691(5) 0.6883(4) 0.1499(2) 0.0485(16) Uani 1 1 d . . . . .
C29 C 0.2910(9) 0.6204(6) 0.2633(4) 0.123(4) Uani 1 1 d . . . . .
C30 C 0.4429(5) 0.6924(4) 0.1332(2) 0.0492(16) Uani 1 1 d . . . . .
C31 C 0.9707(8) 0.6066(6) 0.2565(5) 0.129(4) Uani 1 1 d . . . . .
C32 C 0.8517(8) 0.6106(5) 0.2792(4) 0.104(3) Uani 1 1 d . . . . .
C33 C 0.7788(8) 0.6582(5) 0.2658(4) 0.111(3) Uani 1 1 d . . . . .
C34 C 0.3171(8) 0.3848(5) 0.2177(4) 0.103(3) Uani 1 1 d . . . . .
C35 C 0.4393(9) 0.3854(6) 0.2396(5) 0.135(4) Uani 1 1 d . . . . .
C36 C 0.1483(9) 0.0855(5) 0.2860(4) 0.107(3) Uani 1 1 d . . . . .
C37 C 0.1661(11) 0.1152(7) 0.2364(4) 0.163(6) Uani 1 1 d . . . . .
C38 C 0.0745(12) 0.0247(6) 0.2709(6) 0.172(6) Uani 1 1 d . . . . .
C39 C 0.3235(8) 0.3360(5) 0.5255(5) 0.136(5) Uani 1 1 d . . . . .
C40 C 0.2993(7) 0.2647(5) 0.5164(4) 0.101(3) Uani 1 1 d . . . . .
C41 C 0.2923(9) 0.2441(7) 0.5711(5) 0.141(4) Uani 1 1 d . . . . .
C42 C 0.4139(7) 0.6003(4) 0.2471(3) 0.073(2) Uani 1 1 d . . . . .
C43 C 0.7642(10) 0.9122(5) 0.2166(4) 0.123(4) Uani 1 1 d . . . . .
C44 C 0.7110(13) 0.9716(6) 0.2301(6) 0.168(6) Uani 1 1 d . . . . .
C45 C 0.7864(13) 0.8784(7) 0.2620(5) 0.173(6) Uani 1 1 d . . . . .
C46 C 1.0372(13) 0.7859(13) 0.1697(9) 0.283(12) Uani 1 1 d . . . . .
C47 C 0.797(2) 0.9887(10) 0.0450(11) 0.294(13) Uani 1 1 d . . . . .
C48 C 0.9112(17) 0.6882(8) 0.1220(8) 0.214(8) Uani 1 1 d . . . . .
C49 C 0.3899(16) 0.9107(8) 0.1139(9) 0.205(6) Uani 1 1 d . U . . .
C50 C 0.493(3) 0.9642(15) 0.1039(12) 0.359(14) Uiso 1 1 d . . . . .
C51 C 0.2850(16) 0.9331(10) 0.1265(9) 0.263(9) Uani 1 1 d . U . . .
C52 C 0.4877(13) 0.1672(6) 0.0786(5) 0.144(5) Uani 1 1 d . . . . .
C53 C 0.530(2) 0.1071(11) 0.0589(9) 0.302(13) Uani 1 1 d . U . . .
C54 C 0.8461(9) 0.7452(6) -0.0220(6) 0.141(5) Uani 1 1 d . . . . .
C55 C 0.8642(9) 0.6754(7) -0.0336(6) 0.174(6) Uani 1 1 d . . . . .
C56 C 0.8557(15) 0.7801(10) -0.0628(7) 0.238(10) Uani 1 1 d . . . . .
C57 C -0.0462(11) 0.1674(6) 0.5832(4) 0.123(4) Uani 1 1 d . . . . .
C58 C -0.002(2) 0.1044(9) 0.5834(8) 0.250(10) Uani 1 1 d . U . . .
C59 C -0.0381(17) 0.2123(8) 0.6398(6) 0.225(9) Uani 1 1 d . U . . .
C60 C 0.3724(17) 0.2402(9) 0.3472(9) 0.249(11) Uani 1 1 d . . . . .
C61 C 0.3745(16) 0.3053(9) 0.3697(8) 0.220(9) Uani 1 1 d . . . . .
C62 C 0.4662(16) 0.2030(13) 0.3232(10) 0.324(15) Uani 1 1 d . . . . .
C63 C -0.0894(19) 0.1923(12) 0.1821(8) 0.278(11) Uani 1 1 d . . . . .
C64 C -0.2731(13) 0.1646(11) 0.2235(8) 0.246(9) Uani 1 1 d . U . . .
C65 C -0.1503(15) 0.1644(11) 0.2195(6) 0.228(8) Uani 1 1 d . U . . .
C66 C 0.6952(8) 0.2880(6) 0.0054(4) 0.117(4) Uani 1 1 d . . . . .
C67 C 0.7756(11) 0.2438(10) -0.0178(10) 0.299(14) Uani 1 1 d . . . . .
C68 C 0.7229(10) 0.3298(7) 0.0598(7) 0.203(8) Uani 1 1 d . . . . .
C69 C 0.424(2) 0.1776(13) 0.1307(7) 0.336(15) Uani 1 1 d . U . . .
C70 C -0.3360(9) 0.2432(8) 0.4900(9) 0.283(13) Uani 1 1 d . . . . .
C71 C -0.2537(9) 0.3333(6) 0.5672(6) 0.179(7) Uani 1 1 d . . . . .
C72 C -0.2415(7) 0.2884(5) 0.5106(4) 0.097(3) Uani 1 1 d . . . . .
C73 C -0.1864(8) 0.0944(4) 0.4088(3) 0.091(3) Uani 1 1 d . . . . .
C74 C 0.8640(17) 0.9521(10) 0.0673(10) 0.240(8) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 O11 2.492(4) . ?
La1 O15 2.501(4) . ?
La1 O13 2.527(4) . ?
La1 O12 2.534(4) . ?
La1 O19 2.554(4) . ?
La1 O14 2.557(4) . ?
La1 O18 2.613(4) 2_566 ?
La1 O18 2.701(3) . ?
La1 O41 2.708(4) . ?
La1 N2 3.053(5) . ?
La2 O27 2.474(4) . ?
La2 O22 2.503(4) . ?
La2 O25 2.533(4) . ?
La2 O26 2.543(4) . ?
La2 O23 2.554(4) . ?
La2 O38 2.563(4) . ?
La2 O31 2.617(4) 2_665 ?
La2 O24 2.700(4) . ?
La2 O31 2.707(4) . ?
La2 N1 3.053(6) . ?
Ti1 O4 1.771(4) . ?
Ti1 O3 1.786(5) . ?
Ti1 O6 1.904(4) . ?
Ti1 O5 2.104(4) . ?
Ti1 O16 2.111(4) 2_566 ?
Ti1 O17 2.199(4) 2_566 ?
Ti1 Ti2 3.0956(15) . ?
Ti2 O2 1.762(5) . ?
Ti2 O45 1.771(6) . ?
Ti2 O6 1.947(4) . ?
Ti2 O5 1.968(4) . ?
Ti2 O7 2.023(5) . ?
Ti2 Ti3 3.1245(17) . ?
Ti3 O8 1.775(5) . ?
Ti3 O1 1.797(5) . ?
Ti3 O7 1.995(4) . ?
Ti3 O6 2.040(4) . ?
Ti3 O10 2.068(4) . ?
Ti3 O9 2.180(5) . ?
Ti4 O46 1.744(7) . ?
Ti4 O37 1.779(5) . ?
Ti4 O36 1.972(5) . ?
Ti4 O35 2.054(4) . ?
Ti4 O29 2.062(5) . ?
Ti4 O28 2.167(5) . ?
Ti4 Ti5 3.1289(18) . ?
Ti5 O43 1.755(6) . ?
Ti5 O20 1.772(6) . ?
Ti5 O35 1.940(4) . ?
Ti5 O34 1.963(4) . ?
Ti5 O36 2.020(5) . ?
Ti5 Ti6 3.0877(17) 2_665 ?
Ti6 O32 1.762(5) . ?
Ti6 O33 1.794(5) . ?
Ti6 O35 1.896(4) 2_665 ?
Ti6 O34 2.094(5) 2_665 ?
Ti6 O21 2.115(4) . ?
Ti6 O30 2.209(4) . ?
O1 C73 1.433(9) . ?
O2 C60 1.423(13) . ?
O3 C57 1.437(10) . ?
O4 C72 1.442(9) . ?
O5 C40 1.487(9) . ?
O7 C36 1.469(8) . ?
O8 C65 1.398(14) . ?
O9 C4 1.256(7) . ?
O10 C3 1.275(7) . ?
O11 C4 1.242(7) . ?
O12 C3 1.242(7) . ?
O13 C20 1.477(7) . ?
O14 C17 1.462(8) . ?
O15 C1 1.248(6) . ?
O16 C1 1.251(7) . ?
O17 C2 1.251(6) . ?
O18 C2 1.262(7) . ?
O19 N2 1.274(7) . ?
O20 C23 1.449(15) . ?
O21 C24 1.252(7) . ?
O22 C24 1.233(7) . ?
O23 C5 1.454(8) . ?
O24 N1 1.243(7) . ?
O25 C42 1.461(7) . ?
O26 C30 1.241(7) . ?
O27 C28 1.244(8) . ?
O28 C28 1.256(7) . ?
O29 C30 1.268(8) . ?
O30 C26 1.248(6) . ?
O31 C26 1.254(7) . ?
O32 C66 1.422(10) . ?
O33 C52 1.445(12) . ?
O34 C54 1.483(10) . ?
O36 C43 1.506(9) . ?
O37 C9 1.362(14) . ?
O38 N1 1.278(7) . ?
O39 N1 1.214(7) . ?
O40 C34 1.433(11) . ?
O41 N2 1.237(7) . ?
O42 N2 1.211(6) . ?
O43 C74 1.431(16) . ?
O44 C32 1.465(10) . ?
O45 C8 1.655(19) . ?
O46 C49 1.440(19) . ?
C1 C2 1.558(8) . ?
C3 C4 1.555(8) . ?
C5 C7 1.370(14) . ?
C5 C6 1.452(14) . ?
C8 C11 1.24(3) . ?
C8 C12 1.54(3) . ?
C9 C10 1.26(3) . ?
C9 C14 1.35(3) . ?
C13 C34 1.489(13) . ?
C15 C73 1.569(13) . ?
C16 C73 1.561(12) . ?
C17 C19 1.394(12) . ?
C17 C18 1.502(13) . ?
C20 C22 1.522(11) . ?
C20 C21 1.519(11) . ?
C23 C48 1.401(19) . ?
C23 C46 1.45(2) . ?
C24 C26 1.543(8) . ?
C25 C74 1.36(2) . ?
C27 C42 1.540(11) . ?
C28 C30 1.539(9) . ?
C29 C42 1.547(11) . ?
C31 C32 1.493(13) . ?
C32 C33 1.486(13) . ?
C34 C35 1.516(13) . ?
C36 C38 1.482(14) . ?
C36 C37 1.521(15) . ?
C39 C40 1.512(14) . ?
C40 C41 1.510(14) . ?
C43 C44 1.430(16) . ?
C43 C45 1.513(16) . ?
C47 C74 1.37(2) . ?
C49 C51 1.353(19) . ?
C49 C50 1.68(3) . ?
C52 C53 1.388(19) . ?
C52 C69 1.435(19) . ?
C54 C56 1.40(2) . ?
C54 C55 1.498(17) . ?
C57 C59 1.443(16) . ?
C57 C58 1.50(2) . ?
C60 C61 1.37(2) . ?
C60 C62 1.43(2) . ?
C63 C65 1.39(2) . ?
C64 C65 1.44(2) . ?
C66 C67 1.397(16) . ?
C66 C68 1.399(14) . ?
C70 C72 1.417(14) . ?
C71 C72 1.458(12) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O11 La1 O15 137.48(13) . . ?
O11 La1 O13 84.19(14) . . ?
O15 La1 O13 69.39(13) . . ?
O11 La1 O12 64.94(13) . . ?
O15 La1 O12 136.58(13) . . ?
O13 La1 O12 80.27(14) . . ?
O11 La1 O19 73.19(15) . . ?
O15 La1 O19 94.84(16) . . ?
O13 La1 O19 124.88(14) . . ?
O12 La1 O19 128.32(16) . . ?
O11 La1 O14 137.39(14) . . ?
O15 La1 O14 78.88(15) . . ?
O13 La1 O14 93.73(13) . . ?
O12 La1 O14 72.74(13) . . ?
O19 La1 O14 136.15(13) . . ?
O11 La1 O18 89.79(13) . 2_566 ?
O15 La1 O18 123.96(12) . 2_566 ?
O13 La1 O18 162.95(13) . 2_566 ?
O12 La1 O18 82.73(12) . 2_566 ?
O19 La1 O18 67.82(13) . 2_566 ?
O14 La1 O18 79.94(12) . 2_566 ?
O11 La1 O18 139.19(12) . . ?
O15 La1 O18 63.14(12) . . ?
O13 La1 O18 131.57(13) . . ?
O12 La1 O18 130.36(12) . . ?
O19 La1 O18 69.73(13) . . ?
O14 La1 O18 68.83(11) . . ?
O18 La1 O18 60.86(15) 2_566 . ?
O11 La1 O41 68.40(15) . . ?
O15 La1 O41 73.46(15) . . ?
O13 La1 O41 77.07(14) . . ?
O12 La1 O41 129.57(14) . . ?
O19 La1 O41 47.98(14) . . ?
O14 La1 O41 152.34(16) . . ?
O18 La1 O41 115.44(13) 2_566 . ?
O18 La1 O41 97.65(13) . . ?
O11 La1 N2 67.42(15) . . ?
O15 La1 N2 84.94(16) . . ?
O13 La1 N2 100.66(15) . . ?
O12 La1 N2 131.99(15) . . ?
O19 La1 N2 24.24(15) . . ?
O14 La1 N2 153.00(15) . . ?
O18 La1 N2 91.66(14) 2_566 . ?
O18 La1 N2 84.61(13) . . ?
O41 La1 N2 23.84(14) . . ?
O27 La2 O22 136.67(15) . . ?
O27 La2 O25 84.10(14) . . ?
O22 La2 O25 69.89(13) . . ?
O27 La2 O26 64.68(14) . . ?
O22 La2 O26 137.40(14) . . ?
O25 La2 O26 79.43(14) . . ?
O27 La2 O23 137.64(15) . . ?
O22 La2 O23 79.48(16) . . ?
O25 La2 O23 92.98(13) . . ?
O26 La2 O23 73.22(14) . . ?
O27 La2 O38 73.71(15) . . ?
O22 La2 O38 93.31(17) . . ?
O25 La2 O38 125.21(14) . . ?
O26 La2 O38 128.92(16) . . ?
O23 La2 O38 136.19(13) . . ?
O27 La2 O31 88.86(13) . 2_665 ?
O22 La2 O31 125.09(12) . 2_665 ?
O25 La2 O31 161.68(14) . 2_665 ?
O26 La2 O31 82.26(12) . 2_665 ?
O23 La2 O31 80.88(13) . 2_665 ?
O38 La2 O31 68.20(13) . 2_665 ?
O27 La2 O24 68.45(15) . . ?
O22 La2 O24 72.24(15) . . ?
O25 La2 O24 77.13(14) . . ?
O26 La2 O24 129.10(14) . . ?
O23 La2 O24 151.71(16) . . ?
O38 La2 O24 48.22(14) . . ?
O31 La2 O24 115.85(13) 2_665 . ?
O27 La2 O31 139.49(12) . . ?
O22 La2 O31 62.83(12) . . ?
O25 La2 O31 131.46(13) . . ?
O26 La2 O31 130.96(13) . . ?
O23 La2 O31 68.86(12) . . ?
O38 La2 O31 69.50(13) . . ?
O31 La2 O31 62.26(16) 2_665 . ?
O24 La2 O31 97.77(13) . . ?
O27 La2 N1 67.60(15) . . ?
O22 La2 N1 83.56(17) . . ?
O25 La2 N1 100.85(15) . . ?
O26 La2 N1 131.99(15) . . ?
O23 La2 N1 152.91(15) . . ?
O38 La2 N1 24.36(14) . . ?
O31 La2 N1 91.99(15) 2_665 . ?
O24 La2 N1 23.96(13) . . ?
O31 La2 N1 84.64(13) . . ?
O4 Ti1 O3 97.7(2) . . ?
O4 Ti1 O6 101.07(18) . . ?
O3 Ti1 O6 105.1(2) . . ?
O4 Ti1 O5 170.8(2) . . ?
O3 Ti1 O5 91.3(2) . . ?
O6 Ti1 O5 74.65(16) . . ?
O4 Ti1 O16 92.77(18) . 2_566 ?
O3 Ti1 O16 91.94(19) . 2_566 ?
O6 Ti1 O16 156.17(18) . 2_566 ?
O5 Ti1 O16 88.72(16) . 2_566 ?
O4 Ti1 O17 86.32(19) . 2_566 ?
O3 Ti1 O17 165.92(18) . 2_566 ?
O6 Ti1 O17 87.18(17) . 2_566 ?
O5 Ti1 O17 85.32(17) . 2_566 ?
O16 Ti1 O17 74.35(15) 2_566 2_566 ?
O4 Ti1 Ti2 137.92(14) . . ?
O3 Ti1 Ti2 93.29(16) . . ?
O6 Ti1 Ti2 36.96(12) . . ?
O5 Ti1 Ti2 38.91(12) . . ?
O16 Ti1 Ti2 127.42(12) 2_566 . ?
O17 Ti1 Ti2 92.65(10) 2_566 . ?
O2 Ti2 O45 106.0(3) . . ?
O2 Ti2 O6 138.5(2) . . ?
O45 Ti2 O6 115.5(2) . . ?
O2 Ti2 O5 98.1(2) . . ?
O45 Ti2 O5 101.5(2) . . ?
O6 Ti2 O5 76.93(16) . . ?
O2 Ti2 O7 95.7(2) . . ?
O45 Ti2 O7 98.6(2) . . ?
O6 Ti2 O7 76.09(16) . . ?
O5 Ti2 O7 151.35(18) . . ?
O2 Ti2 Ti1 132.58(18) . . ?
O45 Ti2 Ti1 106.85(18) . . ?
O6 Ti2 Ti1 36.01(11) . . ?
O5 Ti2 Ti1 42.18(12) . . ?
O7 Ti2 Ti1 112.04(13) . . ?
O2 Ti2 Ti3 114.6(2) . . ?
O45 Ti2 Ti3 120.77(19) . . ?
O6 Ti2 Ti3 39.47(12) . . ?
O5 Ti2 Ti3 112.76(13) . . ?
O7 Ti2 Ti3 38.65(12) . . ?
Ti1 Ti2 Ti3 75.00(4) . . ?
O8 Ti3 O1 98.5(2) . . ?
O8 Ti3 O7 100.3(2) . . ?
O1 Ti3 O7 103.7(2) . . ?
O8 Ti3 O6 170.2(2) . . ?
O1 Ti3 O6 91.0(2) . . ?
O7 Ti3 O6 74.66(17) . . ?
O8 Ti3 O10 93.1(2) . . ?
O1 Ti3 O10 96.0(2) . . ?
O7 Ti3 O10 154.05(18) . . ?
O6 Ti3 O10 88.55(16) . . ?
O8 Ti3 O9 90.1(2) . . ?
O1 Ti3 O9 168.91(19) . . ?
O7 Ti3 O9 81.48(18) . . ?
O6 Ti3 O9 80.86(17) . . ?
O10 Ti3 O9 76.34(16) . . ?
O8 Ti3 Ti2 135.19(18) . . ?
O1 Ti3 Ti2 108.22(17) . . ?
O7 Ti3 Ti2 39.30(12) . . ?
O6 Ti3 Ti2 37.34(11) . . ?
O10 Ti3 Ti2 118.25(12) . . ?
O9 Ti3 Ti2 69.51(13) . . ?
O46 Ti4 O37 97.2(3) . . ?
O46 Ti4 O36 104.0(3) . . ?
O37 Ti4 O36 99.8(2) . . ?
O46 Ti4 O35 92.7(2) . . ?
O37 Ti4 O35 169.6(3) . . ?
O36 Ti4 O35 74.48(18) . . ?
O46 Ti4 O29 95.9(3) . . ?
O37 Ti4 O29 94.0(2) . . ?
O36 Ti4 O29 154.1(2) . . ?
O35 Ti4 O29 88.28(17) . . ?
O46 Ti4 O28 170.2(2) . . ?
O37 Ti4 O28 88.8(2) . . ?
O36 Ti4 O28 82.6(2) . . ?
O35 Ti4 O28 81.91(18) . . ?
O29 Ti4 O28 75.81(18) . . ?
O46 Ti4 Ti5 108.6(2) . . ?
O37 Ti4 Ti5 134.8(2) . . ?
O36 Ti4 Ti5 38.95(13) . . ?
O35 Ti4 Ti5 37.16(12) . . ?
O29 Ti4 Ti5 118.57(12) . . ?
O28 Ti4 Ti5 71.75(12) . . ?
O43 Ti5 O20 108.4(3) . . ?
O43 Ti5 O35 115.4(3) . . ?
O20 Ti5 O35 136.0(3) . . ?
O43 Ti5 O34 101.7(2) . . ?
O20 Ti5 O34 98.0(2) . . ?
O35 Ti5 O34 76.85(17) . . ?
O43 Ti5 O36 97.9(2) . . ?
O20 Ti5 O36 95.4(3) . . ?
O35 Ti5 O36 75.93(18) . . ?
O34 Ti5 O36 151.37(19) . . ?
O43 Ti5 Ti6 107.4(2) . 2_665 ?
O20 Ti5 Ti6 130.8(2) . 2_665 ?
O35 Ti5 Ti6 35.91(12) . 2_665 ?
O34 Ti5 Ti6 42.05(13) . 2_665 ?
O36 Ti5 Ti6 111.78(15) . 2_665 ?
O43 Ti5 Ti4 119.2(2) . . ?
O20 Ti5 Ti4 113.4(2) . . ?
O35 Ti5 Ti4 39.75(12) . . ?
O34 Ti5 Ti4 113.56(14) . . ?
O36 Ti5 Ti4 37.85(14) . . ?
Ti6 Ti5 Ti4 75.29(4) 2_665 . ?
O32 Ti6 O33 97.3(2) . . ?
O32 Ti6 O35 102.13(19) . 2_665 ?
O33 Ti6 O35 106.1(2) . 2_665 ?
O32 Ti6 O34 172.2(2) . 2_665 ?
O33 Ti6 O34 90.5(2) . 2_665 ?
O35 Ti6 O34 74.71(18) 2_665 2_665 ?
O32 Ti6 O21 92.35(19) . . ?
O33 Ti6 O21 92.7(2) . . ?
O35 Ti6 O21 154.4(2) 2_665 . ?
O34 Ti6 O21 88.11(17) 2_665 . ?
O32 Ti6 O30 86.34(19) . . ?
O33 Ti6 O30 166.1(2) . . ?
O35 Ti6 O30 86.11(17) 2_665 . ?
O34 Ti6 O30 86.27(18) 2_665 . ?
O21 Ti6 O30 73.69(16) . . ?
O32 Ti6 Ti5 138.90(15) . 2_665 ?
O33 Ti6 Ti5 93.86(18) . 2_665 ?
O35 Ti6 Ti5 36.90(13) 2_665 2_665 ?
O34 Ti6 Ti5 38.89(12) 2_665 2_665 ?
O21 Ti6 Ti5 126.53(13) . 2_665 ?
O30 Ti6 Ti5 92.08(11) . 2_665 ?
C73 O1 Ti3 139.2(4) . . ?
C60 O2 Ti2 161.1(11) . . ?
C57 O3 Ti1 138.1(6) . . ?
C72 O4 Ti1 155.8(5) . . ?
C40 O5 Ti2 121.4(5) . . ?
C40 O5 Ti1 137.5(5) . . ?
Ti2 O5 Ti1 98.91(17) . . ?
Ti1 O6 Ti2 107.03(19) . . ?
Ti1 O6 Ti3 147.6(2) . . ?
Ti2 O6 Ti3 103.19(17) . . ?
C36 O7 Ti3 133.1(5) . . ?
C36 O7 Ti2 124.6(5) . . ?
Ti3 O7 Ti2 102.06(17) . . ?
C65 O8 Ti3 159.7(10) . . ?
C4 O9 Ti3 115.3(4) . . ?
C3 O10 Ti3 118.2(4) . . ?
C4 O11 La1 120.0(4) . . ?
C3 O12 La1 117.7(4) . . ?
C20 O13 La1 127.6(4) . . ?
C17 O14 La1 137.3(5) . . ?
C1 O15 La1 124.6(4) . . ?
C1 O16 Ti1 118.4(4) . 2_566 ?
C2 O17 Ti1 115.7(4) . 2_566 ?
C2 O18 La1 124.1(3) . 2_566 ?
C2 O18 La1 116.5(3) . . ?
La1 O18 La1 119.15(15) 2_566 . ?
N2 O19 La1 100.4(4) . . ?
C23 O20 Ti5 152.7(8) . . ?
C24 O21 Ti6 119.2(4) . . ?
C24 O22 La2 124.4(4) . . ?
C5 O23 La2 136.0(5) . . ?
N1 O24 La2 94.2(4) . . ?
C42 O25 La2 127.4(4) . . ?
C30 O26 La2 117.9(4) . . ?
C28 O27 La2 120.3(4) . . ?
C28 O28 Ti4 116.1(4) . . ?
C30 O29 Ti4 118.4(4) . . ?
C26 O30 Ti6 115.1(4) . . ?
C26 O31 La2 126.0(3) . 2_665 ?
C26 O31 La2 116.1(3) . . ?
La2 O31 La2 117.74(16) 2_665 . ?
C66 O32 Ti6 158.6(6) . . ?
C52 O33 Ti6 135.5(7) . . ?
C54 O34 Ti5 122.9(5) . . ?
C54 O34 Ti6 135.5(6) . 2_665 ?
Ti5 O34 Ti6 99.07(19) . 2_665 ?
Ti6 O35 Ti5 107.19(19) 2_665 . ?
Ti6 O35 Ti4 148.0(2) 2_665 . ?
Ti5 O35 Ti4 103.09(19) . . ?
C43 O36 Ti4 134.6(5) . . ?
C43 O36 Ti5 122.0(5) . . ?
Ti4 O36 Ti5 103.2(2) . . ?
C9 O37 Ti4 159.6(12) . . ?
N1 O38 La2 99.8(4) . . ?
N2 O41 La1 93.9(3) . . ?
C74 O43 Ti5 170.2(10) . . ?
C8 O45 Ti2 173.1(8) . . ?
C49 O46 Ti4 151.6(9) . . ?
O39 N1 O24 123.5(6) . . ?
O39 N1 O38 119.2(6) . . ?
O24 N1 O38 117.3(5) . . ?
O39 N1 La2 171.6(6) . . ?
O24 N1 La2 61.9(3) . . ?
O38 N1 La2 55.8(3) . . ?
O42 N2 O41 123.1(6) . . ?
O42 N2 O19 119.6(6) . . ?
O41 N2 O19 117.3(5) . . ?
O42 N2 La1 171.2(6) . . ?
O41 N2 La1 62.2(3) . . ?
O19 N2 La1 55.4(3) . . ?
O15 C1 O16 127.2(5) . . ?
O15 C1 C2 117.4(6) . . ?
O16 C1 C2 115.4(5) . . ?
O17 C2 O18 127.8(5) . . ?
O17 C2 C1 114.1(5) . . ?
O18 C2 C1 118.1(5) . . ?
O12 C3 O10 126.8(5) . . ?
O12 C3 C4 117.9(6) . . ?
O10 C3 C4 115.2(6) . . ?
O11 C4 O9 128.2(6) . . ?
O11 C4 C3 116.9(6) . . ?
O9 C4 C3 114.9(6) . . ?
C7 C5 C6 129.8(9) . . ?
C7 C5 O23 113.8(9) . . ?
C6 C5 O23 112.0(8) . . ?
C11 C8 C12 96(2) . . ?
C11 C8 O45 98(2) . . ?
C12 C8 O45 88.9(18) . . ?
C10 C9 C14 119(2) . . ?
C10 C9 O37 121(2) . . ?
C14 C9 O37 119(2) . . ?
C19 C17 O14 113.3(7) . . ?
C19 C17 C18 126.4(9) . . ?
O14 C17 C18 109.8(8) . . ?
O13 C20 C22 108.3(6) . . ?
O13 C20 C21 108.4(6) . . ?
C22 C20 C21 112.4(7) . . ?
C48 C23 O20 113.0(14) . . ?
C48 C23 C46 121.5(18) . . ?
O20 C23 C46 103.6(15) . . ?
O22 C24 O21 127.4(5) . . ?
O22 C24 C26 118.2(6) . . ?
O21 C24 C26 114.4(5) . . ?
O30 C26 O31 126.6(5) . . ?
O30 C26 C24 115.2(5) . . ?
O31 C26 C24 118.2(5) . . ?
O27 C28 O28 128.5(6) . . ?
O27 C28 C30 117.4(6) . . ?
O28 C28 C30 114.1(6) . . ?
O26 C30 O29 127.0(6) . . ?
O26 C30 C28 117.5(6) . . ?
O29 C30 C28 115.5(6) . . ?
O44 C32 C33 113.8(7) . . ?
O44 C32 C31 109.4(8) . . ?
C33 C32 C31 118.2(10) . . ?
O40 C34 C13 114.1(8) . . ?
O40 C34 C35 110.2(9) . . ?
C13 C34 C35 117.5(10) . . ?
O7 C36 C38 109.2(8) . . ?
O7 C36 C37 108.7(8) . . ?
C38 C36 C37 113.9(10) . . ?
O5 C40 C41 108.3(8) . . ?
O5 C40 C39 108.7(8) . . ?
C41 C40 C39 114.6(9) . . ?
O25 C42 C27 109.0(7) . . ?
O25 C42 C29 108.0(6) . . ?
C27 C42 C29 111.7(7) . . ?
C44 C43 C45 121.6(11) . . ?
C44 C43 O36 107.2(10) . . ?
C45 C43 O36 107.1(8) . . ?
C51 C49 O46 121.3(19) . . ?
C51 C49 C50 116(2) . . ?
O46 C49 C50 101.1(16) . . ?
C53 C52 C69 115.5(16) . . ?
C53 C52 O33 115.2(12) . . ?
C69 C52 O33 106.8(13) . . ?
C56 C54 O34 112.1(13) . . ?
C56 C54 C55 125.3(13) . . ?
O34 C54 C55 110.2(9) . . ?
O3 C57 C59 112.4(10) . . ?
O3 C57 C58 105.9(10) . . ?
C59 C57 C58 111.5(13) . . ?
C61 C60 O2 113.3(14) . . ?
C61 C60 C62 127.5(18) . . ?
O2 C60 C62 109.5(17) . . ?
O8 C65 C63 118.3(16) . . ?
O8 C65 C64 115.1(13) . . ?
C63 C65 C64 122.1(18) . . ?
C67 C66 C68 116.1(11) . . ?
C67 C66 O32 109.6(11) . . ?
C68 C66 O32 113.1(10) . . ?
C70 C72 O4 109.2(9) . . ?
C70 C72 C71 116.2(10) . . ?
O4 C72 C71 111.9(8) . . ?
O1 C73 C16 105.9(8) . . ?
O1 C73 C15 108.6(7) . . ?
C16 C73 C15 113.9(8) . . ?
C25 C74 C47 130(2) . . ?
C25 C74 O43 114.3(19) . . ?
C47 C74 O43 115.4(18) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O8 Ti3 O1 C73 -175.8(8) . . . . ?
O7 Ti3 O1 C73 81.4(8) . . . . ?
O6 Ti3 O1 C73 7.0(8) . . . . ?
O10 Ti3 O1 C73 -81.7(8) . . . . ?
O9 Ti3 O1 C73 -35.6(16) . . . . ?
Ti2 Ti3 O1 C73 40.7(8) . . . . ?
O45 Ti2 O2 C60 167(3) . . . . ?
O6 Ti2 O2 C60 -9(3) . . . . ?
O5 Ti2 O2 C60 -89(3) . . . . ?
O7 Ti2 O2 C60 66(3) . . . . ?
Ti1 Ti2 O2 C60 -61(3) . . . . ?
Ti3 Ti2 O2 C60 31(3) . . . . ?
O4 Ti1 O3 C57 -18.5(9) . . . . ?
O6 Ti1 O3 C57 -122.2(8) . . . . ?
O5 Ti1 O3 C57 163.3(8) . . . . ?
O16 Ti1 O3 C57 74.6(9) 2_566 . . . ?
O17 Ti1 O3 C57 87.5(12) 2_566 . . . ?
Ti2 Ti1 O3 C57 -157.8(8) . . . . ?
O3 Ti1 O4 C72 150.1(11) . . . . ?
O6 Ti1 O4 C72 -102.7(11) . . . . ?
O16 Ti1 O4 C72 57.8(11) 2_566 . . . ?
O17 Ti1 O4 C72 -16.3(11) 2_566 . . . ?
Ti2 Ti1 O4 C72 -106.2(10) . . . . ?
O1 Ti3 O8 C65 91(3) . . . . ?
O7 Ti3 O8 C65 -163(3) . . . . ?
O10 Ti3 O8 C65 -5(3) . . . . ?
O9 Ti3 O8 C65 -82(3) . . . . ?
Ti2 Ti3 O8 C65 -142(3) . . . . ?
O43 Ti5 O20 C23 161.6(18) . . . . ?
O35 Ti5 O20 C23 -14(2) . . . . ?
O34 Ti5 O20 C23 -93.2(19) . . . . ?
O36 Ti5 O20 C23 61.5(19) . . . . ?
Ti6 Ti5 O20 C23 -63.6(19) 2_665 . . . ?
Ti4 Ti5 O20 C23 26.9(19) . . . . ?
O33 Ti6 O32 C66 -148.6(14) . . . . ?
O35 Ti6 O32 C66 103.1(14) 2_665 . . . ?
O21 Ti6 O32 C66 -55.6(14) . . . . ?
O30 Ti6 O32 C66 17.9(14) . . . . ?
Ti5 Ti6 O32 C66 106.9(14) 2_665 . . . ?
O32 Ti6 O33 C52 20.8(10) . . . . ?
O35 Ti6 O33 C52 125.8(9) 2_665 . . . ?
O34 Ti6 O33 C52 -160.0(9) 2_665 . . . ?
O21 Ti6 O33 C52 -71.9(10) . . . . ?
O30 Ti6 O33 C52 -83.8(13) . . . . ?
Ti5 Ti6 O33 C52 161.2(9) 2_665 . . . ?
O46 Ti4 O37 C9 56(4) . . . . ?
O36 Ti4 O37 C9 161(4) . . . . ?
O35 Ti4 O37 C9 -143(4) . . . . ?
O29 Ti4 O37 C9 -41(4) . . . . ?
O28 Ti4 O37 C9 -116(4) . . . . ?
Ti5 Ti4 O37 C9 -179(4) . . . . ?
O37 Ti4 O46 C49 -165.7(19) . . . . ?
O36 Ti4 O46 C49 92.4(19) . . . . ?
O35 Ti4 O46 C49 17.7(19) . . . . ?
O29 Ti4 O46 C49 -70.9(19) . . . . ?
Ti5 Ti4 O46 C49 52.0(19) . . . . ?
La2 O24 N1 O39 172.5(7) . . . . ?
La2 O24 N1 O38 -6.7(6) . . . . ?
La2 O38 N1 O39 -172.1(6) . . . . ?
La2 O38 N1 O24 7.1(7) . . . . ?
La1 O41 N2 O42 171.8(7) . . . . ?
La1 O41 N2 O19 -6.2(6) . . . . ?
La1 O19 N2 O42 -171.4(6) . . . . ?
La1 O19 N2 O41 6.6(7) . . . . ?
La1 O15 C1 O16 178.4(4) . . . . ?
La1 O15 C1 C2 -1.3(7) . . . . ?
Ti1 O16 C1 O15 -172.2(5) 2_566 . . . ?
Ti1 O16 C1 C2 7.5(6) 2_566 . . . ?
Ti1 O17 C2 O18 165.8(4) 2_566 . . . ?
Ti1 O17 C2 C1 -13.4(5) 2_566 . . . ?
La1 O18 C2 O17 1.1(7) 2_566 . . . ?
La1 O18 C2 O17 175.3(4) . . . . ?
La1 O18 C2 C1 -179.7(3) 2_566 . . . ?
La1 O18 C2 C1 -5.5(6) . . . . ?
O15 C1 C2 O17 -175.9(5) . . . . ?
O16 C1 C2 O17 4.4(7) . . . . ?
O15 C1 C2 O18 4.8(7) . . . . ?
O16 C1 C2 O18 -174.9(5) . . . . ?
La1 O12 C3 O10 168.6(4) . . . . ?
La1 O12 C3 C4 -13.3(6) . . . . ?
Ti3 O10 C3 O12 178.9(4) . . . . ?
Ti3 O10 C3 C4 0.8(6) . . . . ?
La1 O11 C4 O9 -168.8(5) . . . . ?
La1 O11 C4 C3 11.8(7) . . . . ?
Ti3 O9 C4 O11 179.6(5) . . . . ?
Ti3 O9 C4 C3 -0.9(6) . . . . ?
O12 C3 C4 O11 1.3(8) . . . . ?
O10 C3 C4 O11 179.6(5) . . . . ?
O12 C3 C4 O9 -178.2(5) . . . . ?
O10 C3 C4 O9 0.1(7) . . . . ?
La2 O23 C5 C7 -51.3(15) . . . . ?
La2 O23 C5 C6 107.8(9) . . . . ?
Ti4 O37 C9 C10 6(7) . . . . ?
Ti4 O37 C9 C14 172(3) . . . . ?
La1 O14 C17 C19 -39.0(14) . . . . ?
La1 O14 C17 C18 108.4(8) . . . . ?
La1 O13 C20 C22 115.1(6) . . . . ?
La1 O13 C20 C21 -122.6(6) . . . . ?
Ti5 O20 C23 C48 72(3) . . . . ?
Ti5 O20 C23 C46 -154.9(14) . . . . ?
La2 O22 C24 O21 177.6(5) . . . . ?
La2 O22 C24 C26 -2.0(8) . . . . ?
Ti6 O21 C24 O22 -172.2(5) . . . . ?
Ti6 O21 C24 C26 7.3(7) . . . . ?
Ti6 O30 C26 O31 165.0(5) . . . . ?
Ti6 O30 C26 C24 -15.0(6) . . . . ?
La2 O31 C26 O30 -1.2(8) 2_665 . . . ?
La2 O31 C26 O30 174.4(4) . . . . ?
La2 O31 C26 C24 178.7(3) 2_665 . . . ?
La2 O31 C26 C24 -5.7(6) . . . . ?
O22 C24 C26 O30 -174.6(5) . . . . ?
O21 C24 C26 O30 5.7(8) . . . . ?
O22 C24 C26 O31 5.4(8) . . . . ?
O21 C24 C26 O31 -174.2(5) . . . . ?
La2 O27 C28 O28 -169.0(5) . . . . ?
La2 O27 C28 C30 12.1(7) . . . . ?
Ti4 O28 C28 O27 179.2(5) . . . . ?
Ti4 O28 C28 C30 -1.9(6) . . . . ?
La2 O26 C30 O29 169.0(5) . . . . ?
La2 O26 C30 C28 -11.7(7) . . . . ?
Ti4 O29 C30 O26 -179.3(5) . . . . ?
Ti4 O29 C30 C28 1.3(7) . . . . ?
O27 C28 C30 O26 0.1(8) . . . . ?
O28 C28 C30 O26 -178.9(5) . . . . ?
O27 C28 C30 O29 179.5(5) . . . . ?
O28 C28 C30 O29 0.5(8) . . . . ?
Ti3 O7 C36 C38 -62.2(12) . . . . ?
Ti2 O7 C36 C38 124.8(9) . . . . ?
Ti3 O7 C36 C37 62.6(11) . . . . ?
Ti2 O7 C36 C37 -110.4(9) . . . . ?
Ti2 O5 C40 C41 -113.3(8) . . . . ?
Ti1 O5 C40 C41 46.1(12) . . . . ?
Ti2 O5 C40 C39 121.5(7) . . . . ?
Ti1 O5 C40 C39 -79.1(11) . . . . ?
La2 O25 C42 C27 -123.3(5) . . . . ?
La2 O25 C42 C29 115.3(6) . . . . ?
Ti4 O36 C43 C44 -66.0(12) . . . . ?
Ti5 O36 C43 C44 119.7(9) . . . . ?
Ti4 O36 C43 C45 66.1(13) . . . . ?
Ti5 O36 C43 C45 -108.3(9) . . . . ?
Ti4 O46 C49 C51 141.2(17) . . . . ?
Ti4 O46 C49 C50 -89(2) . . . . ?
Ti6 O33 C52 C53 -111.0(17) . . . . ?
Ti6 O33 C52 C69 119.4(15) . . . . ?
Ti5 O34 C54 C56 -96.5(13) . . . . ?
Ti6 O34 C54 C56 61.5(14) 2_665 . . . ?
Ti5 O34 C54 C55 119.0(9) . . . . ?
Ti6 O34 C54 C55 -83.0(14) 2_665 . . . ?
Ti1 O3 C57 C59 -76.2(15) . . . . ?
Ti1 O3 C57 C58 161.8(10) . . . . ?
Ti2 O2 C60 C61 61(4) . . . . ?
Ti2 O2 C60 C62 -151(2) . . . . ?
Ti3 O8 C65 C63 109(2) . . . . ?
Ti3 O8 C65 C64 -48(4) . . . . ?
Ti6 O32 C66 C67 -152.9(15) . . . . ?
Ti6 O32 C66 C68 75.8(19) . . . . ?
Ti1 O4 C72 C70 153.0(13) . . . . ?
Ti1 O4 C72 C71 -77.0(15) . . . . ?
Ti3 O1 C73 C16 149.9(7) . . . . ?
Ti3 O1 C73 C15 -87.5(9) . . . . ?

_refine_diff_density_max         1.156
_refine_diff_density_min         -0.732
_refine_diff_density_rms         0.106
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_2
_database_code_depnum_ccdc_archive 'CCDC 1828905'
_audit_update_record             
;
2018-03-13 deposited with the CCDC.
2018-05-31 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C74 H156 Ce2 N2 O46 Ti6'
_chemical_formula_weight         2377.45

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ti Ti 0.2776 0.4457 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.3596(6)
_cell_length_b                   21.1998(12)
_cell_length_c                   23.9317(13)
_cell_angle_alpha                105.4150(10)
_cell_angle_beta                 90.3820(10)
_cell_angle_gamma                94.5150(10)
_cell_volume                     5536.4(5)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    7354
_cell_measurement_theta_min      2.6
_cell_measurement_theta_max      25.2

_exptl_crystal_description       block
_exptl_crystal_colour            'light yellow'
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    1.431
_exptl_crystal_F_000             2460
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.350
_exptl_crystal_size_mid          0.200
_exptl_crystal_size_min          0.150
_exptl_absorpt_coefficient_mu    1.296
_shelx_estimated_absorpt_T_min   0.660
_shelx_estimated_absorpt_T_max   0.829
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.352
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Xcalibur, Atlas, Gemini'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            28280
_diffrn_reflns_av_unetI/netI     0.0788
_diffrn_reflns_av_R_equivalents  0.0359
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_theta_min         0.883
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_full        25.000
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measured_fraction_theta_full 0.991
_diffrn_reflns_Laue_measured_fraction_max 0.991
_diffrn_reflns_Laue_measured_fraction_full 0.991
_diffrn_reflns_point_group_measured_fraction_max 0.991
_diffrn_reflns_point_group_measured_fraction_full 0.991
_reflns_number_total             19365
_reflns_number_gt                14081
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0773P)²+27.5066P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         19365
_refine_ls_number_parameters     1171
_refine_ls_number_restraints     39
_refine_ls_R_factor_all          0.0855
_refine_ls_R_factor_gt           0.0564
_refine_ls_wR_factor_ref         0.1655
_refine_ls_wR_factor_gt          0.1418
_refine_ls_goodness_of_fit_ref   1.022
_refine_ls_restrained_S_all      1.024
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ce1 Ce 0.03682(3) 0.04116(2) 0.59771(2) 0.01030(11) Uani 1 1 d . . . . .
Ce2 Ce 0.47438(3) 0.03557(2) 0.09695(2) 0.01030(11) Uani 1 1 d . . . . .
Ti1 Ti 0.55992(11) 0.26133(6) 0.00190(5) 0.0126(3) Uani 1 1 d . . . . .
Ti2 Ti 0.00872(11) 0.25723(6) 0.49404(5) 0.0125(3) Uani 1 1 d . . . . .
Ti3 Ti 0.06650(11) 0.33414(6) 0.65406(5) 0.0142(3) Uani 1 1 d . . . . .
Ti4 Ti 0.52316(12) 0.32826(6) 0.16410(5) 0.0159(3) Uani 1 1 d . . . . .
Ti5 Ti 0.75165(11) 0.33158(6) 0.09331(5) 0.0155(3) Uani 1 1 d . . . . .
Ti6 Ti -0.16787(11) 0.32526(6) 0.58293(5) 0.0145(3) Uani 1 1 d . . . . .
O1 O 0.6019(4) 0.1352(2) 0.14270(19) 0.0162(10) Uani 1 1 d . . . . .
O2 O 0.3707(4) 0.1384(2) 0.11756(19) 0.0140(10) Uani 1 1 d . . . . .
O3 O 0.6834(4) 0.0148(3) 0.0665(2) 0.0229(12) Uani 1 1 d . . . . .
O4 O 0.4371(4) -0.0754(2) 0.10946(19) 0.0163(11) Uani 1 1 d . . . . .
O5 O 0.2757(4) 0.0022(2) 0.0467(2) 0.0182(11) Uani 1 1 d . . . . .
O6 O 0.4072(4) 0.0435(2) 0.19734(19) 0.0155(10) Uani 1 1 d . . . . .
O7 O 0.5530(4) 0.1725(2) 0.03133(19) 0.0143(10) Uani 1 1 d . . . . .
O8 O 0.5184(4) 0.0630(2) -0.00099(18) 0.0125(10) Uani 1 1 d . . . . .
O9 O 0.5794(4) 0.1843(2) -0.07263(19) 0.0158(10) Uani 1 1 d . . . . .
O10 O 0.5764(4) 0.3204(2) -0.0400(2) 0.0193(11) Uani 1 1 d . . . . .
O11 O 0.7415(4) 0.2659(2) 0.01748(19) 0.0166(11) Uani 1 1 d . . . . .
O12 O 0.5822(4) 0.3094(2) 0.08069(19) 0.0142(10) Uani 1 1 d . . . . .
O13 O 0.4277(5) 0.3851(2) 0.1494(2) 0.0222(12) Uani 1 1 d . . . . .
O14 O 0.6834(4) 0.3744(2) 0.1705(2) 0.0187(11) Uani 1 1 d . . . . .
O15 O 0.6227(4) 0.2450(2) 0.16369(19) 0.0154(10) Uani 1 1 d . . . . .
O16 O 0.3997(4) 0.2485(2) 0.1375(2) 0.0162(10) Uani 1 1 d . . . . .
O17 O 0.4965(5) 0.3411(2) 0.2389(2) 0.0223(12) Uani 1 1 d . . . . .
O18 O 0.8717(4) 0.3020(2) 0.1242(2) 0.0217(11) Uani 1 1 d . . . . .
O19 O 0.8052(5) 0.4032(2) 0.0741(2) 0.0261(12) Uani 1 1 d . U . . .
O20 O 0.4021(4) 0.2472(2) -0.0040(2) 0.0171(11) Uani 1 1 d . . . . .
O21 O -0.0026(4) 0.1704(2) 0.52677(19) 0.0154(10) Uani 1 1 d . . . . .
O22 O -0.0022(4) 0.3082(2) 0.57177(18) 0.0133(10) Uani 1 1 d . . . . .
O23 O 0.0023(4) 0.0611(2) 0.49732(19) 0.0131(10) Uani 1 1 d . . . . .
O24 O 0.0033(4) 0.3152(2) 0.45208(19) 0.0158(10) Uani 1 1 d . . . . .
O25 O -0.0608(4) 0.1410(2) 0.64270(19) 0.0154(10) Uani 1 1 d . . . . .
O26 O -0.0317(4) 0.1778(2) 0.42109(19) 0.0149(10) Uani 1 1 d . . . . .
O27 O -0.1790(4) 0.0214(3) 0.56756(19) 0.0224(12) Uani 1 1 d . . . . .
O28 O -0.1595(4) 0.0185(2) 0.65631(19) 0.0169(11) Uani 1 1 d . . . . .
O29 O 0.1690(4) 0.1456(2) 0.61566(19) 0.0144(10) Uani 1 1 d . . . . .
O30 O -0.0848(4) 0.3755(2) 0.65910(19) 0.0177(11) Uani 1 1 d . . . . .
O31 O 0.0408(4) -0.0684(2) 0.61281(19) 0.0172(11) Uani 1 1 d . . . . .
O32 O 0.2253(4) 0.0071(2) 0.5482(2) 0.0175(11) Uani 1 1 d . . . . .
O33 O 0.1726(4) 0.3927(2) 0.6361(2) 0.0179(11) Uani 1 1 d . . . . .
O34 O 0.1643(4) 0.2482(2) 0.4895(2) 0.0171(11) Uani 1 1 d . . . . .
O35 O -0.1720(4) 0.2564(2) 0.5092(2) 0.0162(10) Uani 1 1 d . . . . .
O36 O -0.2186(4) 0.3914(2) 0.5588(2) 0.0200(11) Uani 1 1 d . . . . .
O37 O 0.1067(4) 0.3487(2) 0.7286(2) 0.0229(12) Uani 1 1 d . . . . .
O38 O -0.2918(4) 0.2954(2) 0.6159(2) 0.0201(11) Uani 1 1 d . . . . .
O39 O 0.7226(4) 0.0554(2) 0.7703(2) 0.0208(11) Uani 1 1 d . . . . .
O40 O 0.1108(4) 0.0509(2) 0.69798(19) 0.0150(10) Uani 1 1 d . . . . .
O41 O 0.1686(4) 0.2552(2) 0.62984(19) 0.0149(10) Uani 1 1 d . . . . .
O42 O -0.0529(4) 0.2504(2) 0.65883(19) 0.0153(10) Uani 1 1 d . . . . .
O43 O -0.3349(5) 0.0191(3) 0.6199(2) 0.0294(13) Uani 1 1 d . . . . .
O44 O 0.7881(4) 0.0459(2) 0.2695(2) 0.0190(11) Uani 1 1 d . . . . .
O46 O 0.6635(4) 0.0101(2) 0.1546(2) 0.0168(11) Uani 1 1 d . . . . .
O47 O 0.8397(5) 0.0095(3) 0.1180(2) 0.0296(13) Uani 1 1 d . . . . .
N1 N -0.2278(5) 0.0199(3) 0.6155(3) 0.0195(14) Uani 1 1 d . . . . .
N2 N 0.7333(5) 0.0112(3) 0.1141(2) 0.0175(13) Uani 1 1 d . . . . .
C1 C 0.5089(8) 0.3277(4) -0.0881(3) 0.0291(19) Uani 1 1 d . . . . .
C2 C 0.5943(8) 0.3495(5) -0.1299(3) 0.036(2) Uani 1 1 d . . . . .
C3 C 0.4156(8) 0.3753(4) -0.0664(4) 0.033(2) Uani 1 1 d . . . . .
C4 C 0.2972(7) 0.2050(4) -0.0052(3) 0.0217(17) Uani 1 1 d . . . . .
C5 C 0.2016(7) 0.2475(4) 0.0275(4) 0.031(2) Uani 1 1 d . . . . .
C6 C 0.5635(6) 0.1260(3) -0.0693(3) 0.0136(15) Uani 1 1 d . . . . .
C7 C 0.5435(6) 0.1196(3) -0.0071(3) 0.0120(14) Uani 1 1 d . . . . .
C8 C 0.4298(9) 0.3663(5) 0.2897(4) 0.045(3) Uani 1 1 d . . . . .
C9 C 0.4455(12) 0.3260(7) 0.3312(5) 0.077(4) Uani 1 1 d . . . . .
C10 C 0.7500(7) 0.4220(4) 0.2165(3) 0.0242(18) Uani 1 1 d . . . . .
C11 C 0.7681(8) 0.3949(4) 0.2688(3) 0.033(2) Uani 1 1 d . . . . .
C12 C 0.6894(9) 0.4853(4) 0.2314(4) 0.038(2) Uani 1 1 d . . . . .
C13 C 0.5650(6) 0.1902(3) 0.1476(3) 0.0136(15) Uani 1 1 d . . . . .
C14 C 0.4323(6) 0.1917(3) 0.1323(3) 0.0143(15) Uani 1 1 d . . . . .
C15 C 0.9596(10) 0.4872(6) 0.1058(6) 0.078(4) Uani 1 1 d . U . . .
C16 C 0.8475(7) 0.2511(4) -0.0162(3) 0.0224(17) Uani 1 1 d . . . . .
C17 C 0.8476(8) 0.2813(5) -0.0662(4) 0.037(2) Uani 1 1 d . . . . .
C18 C 0.8569(7) 0.1773(4) -0.0355(4) 0.0303(19) Uani 1 1 d . . . . .
C19 C 0.1497(6) 0.0057(4) 0.0617(3) 0.0165(15) Uani 1 1 d . U . . .
C20 C 0.1423(7) 0.0080(4) 0.1248(3) 0.0287(19) Uani 1 1 d . . . . .
C21 C 0.1026(7) 0.0648(4) 0.0465(3) 0.0259(18) Uani 1 1 d . . . . .
C22 C 0.9101(7) 0.2631(4) 0.1598(3) 0.0257(18) Uani 1 1 d . . . . .
C23 C 1.0294(8) 0.2919(5) 0.1877(4) 0.044(3) Uani 1 1 d . . . . .
C24 C 0.4191(6) 0.1005(4) 0.2476(3) 0.0189(16) Uani 1 1 d . . . . .
C25 C 0.4770(7) 0.0813(4) 0.2982(3) 0.0243(17) Uani 1 1 d . . . . .
C26 C 0.2623(6) 0.2103(4) 0.4919(3) 0.0202(16) Uani 1 1 d . . . . .
C27 C 0.3661(8) 0.2563(4) 0.5218(4) 0.035(2) Uani 1 1 d . . . . .
C28 C 0.2886(8) 0.1720(4) 0.4300(4) 0.037(2) Uani 1 1 d . . . . .
C29 C 0.0718(7) 0.3376(4) 0.4103(3) 0.0246(18) Uani 1 1 d . . . . .
C30 C 0.0163(9) 0.3970(4) 0.4007(4) 0.041(2) Uani 1 1 d . . . . .
C31 C -0.0282(6) 0.1202(3) 0.4262(3) 0.0124(14) Uani 1 1 d . . . . .
C32 C -0.0080(6) 0.1164(3) 0.4889(3) 0.0112(14) Uani 1 1 d . . . . .
C33 C -0.2798(7) 0.2373(4) 0.4738(3) 0.0240(17) Uani 1 1 d . . . . .
C34 C -0.3128(7) 0.1635(4) 0.4628(4) 0.0298(19) Uani 1 1 d . . . . .
C35 C -0.2675(7) 0.2583(4) 0.4177(3) 0.0290(19) Uani 1 1 d . . . . .
C36 C -0.1404(7) 0.4230(4) 0.7043(3) 0.0234(17) Uani 1 1 d . . . . .
C37 C -0.0643(8) 0.4873(4) 0.7183(4) 0.035(2) Uani 1 1 d . . . . .
C38 C -0.1567(8) 0.3967(4) 0.7581(3) 0.033(2) Uani 1 1 d . . . . .
C39 C 0.1626(10) 0.3406(8) 0.7778(4) 0.072(4) Uani 1 1 d . U . . .
C40 C -0.0108(6) 0.1959(3) 0.6444(3) 0.0147(15) Uani 1 1 d . . . . .
C41 C 0.1208(6) 0.1980(3) 0.6286(3) 0.0137(15) Uani 1 1 d . . . . .
C42 C -0.3267(7) 0.4219(4) 0.5594(3) 0.0289(19) Uani 1 1 d . . . . .
C43 C -0.3725(8) 0.4114(5) 0.4965(4) 0.039(2) Uani 1 1 d . . . . .
C44 C -0.3028(10) 0.4943(5) 0.5897(5) 0.059(3) Uani 1 1 d . . . . .
C45 C -0.3377(7) 0.2603(4) 0.6558(3) 0.0230(17) Uani 1 1 d . . . . .
C46 C -0.3674(9) 0.1885(4) 0.6212(4) 0.040(2) Uani 1 1 d . . . . .
C47 C 0.3519(6) 0.0136(4) 0.5621(3) 0.0178(15) Uani 1 1 d . . . . .
C48 C 0.3665(7) 0.0266(4) 0.6270(3) 0.0280(19) Uani 1 1 d . . . . .
C49 C 0.1129(7) 0.1079(3) 0.7487(3) 0.0177(16) Uani 1 1 d . . . . .
C50 C 0.2421(7) 0.1334(4) 0.7650(3) 0.0261(18) Uani 1 1 d . . . . .
C51 C 0.0486(7) 0.0890(4) 0.7981(3) 0.0234(17) Uani 1 1 d . . . . .
C52 C 0.2979(7) 0.1261(4) 0.2623(3) 0.0276(19) Uani 1 1 d . . . . .
C53 C 0.2590(8) 0.1722(4) -0.0683(4) 0.036(2) Uani 1 1 d . . . . .
C54 C 0.9131(8) 0.1915(4) 0.1219(4) 0.037(2) Uani 1 1 d . . . . .
C55 C 0.0873(10) 0.3060(6) 0.8115(5) 0.063(3) Uani 1 1 d . . . . .
C56 C 0.3051(9) 0.3714(6) 0.2722(4) 0.060(3) Uani 1 1 d . . . . .
C57 C 0.4122(7) 0.0678(4) 0.5384(3) 0.0253(18) Uani 1 1 d . . . . .
C58 C -0.4461(8) 0.2925(5) 0.6831(4) 0.045(2) Uani 1 1 d . . . . .
C59 C 0.2868(8) 0.3244(5) 0.7679(4) 0.047(3) Uani 1 1 d . . . . .
C60 C 0.8496(6) 0.1106(4) 0.2814(3) 0.0208(16) Uani 1 1 d . . . . .
C61 C 0.9721(7) 0.1061(4) 0.2567(3) 0.0306(19) Uani 1 1 d . . . . .
C62 C 0.7768(7) 0.1577(4) 0.2602(3) 0.0230(17) Uani 1 1 d . . . . .
C63 C 0.6888(6) 0.1223(4) 0.7877(3) 0.0191(16) Uani 1 1 d . . . . .
C64 C 0.7751(7) 0.1682(4) 0.7654(3) 0.0263(18) Uani 1 1 d . . . . .
C65 C 0.5596(7) 0.1229(4) 0.7673(4) 0.032(2) Uani 1 1 d . . . . .
C66 C 0.2110(7) 0.4101(4) 0.5846(3) 0.0222(17) Uani 1 1 d . . . . .
C67 C 0.3854(7) 0.4068(4) 0.1015(3) 0.0264(18) Uani 1 1 d . . . . .
C68 C 0.1297(8) 0.4571(4) 0.5712(4) 0.0292(19) Uani 1 1 d . . . . .
C69 C 0.3402(8) 0.4400(4) 0.5963(4) 0.037(2) Uani 1 1 d . . . . .
C70 C 0.4734(9) 0.4624(4) 0.0934(4) 0.041(2) Uani 1 1 d . . . . .
C71 C 0.2614(9) 0.4291(5) 0.1149(4) 0.046(3) Uani 1 1 d . . . . .
C72 C 0.8128(12) 0.4884(6) 0.0258(6) 0.077(4) Uani 1 1 d . U . . .
C73 C 0.8797(12) 0.4517(6) 0.0604(5) 0.076(4) Uani 1 1 d . U . . .
C74 C 0.0721(9) 0.2814(4) 0.3535(3) 0.041(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ce1 O31 2.447(5) . ?
Ce1 O25 2.458(4) . ?
Ce1 O40 2.488(4) . ?
Ce1 O29 2.512(5) . ?
Ce1 O32 2.516(5) . ?
Ce1 O27 2.522(5) . ?
Ce1 O23 2.580(4) . ?
Ce1 O23 2.699(4) 2_556 ?
Ce1 O28 2.720(5) . ?
Ce2 O4 2.453(5) . ?
Ce2 O1 2.454(5) . ?
Ce2 O6 2.492(4) . ?
Ce2 O2 2.495(4) . ?
Ce2 O5 2.510(5) . ?
Ce2 O3 2.526(5) . ?
Ce2 O8 2.603(4) . ?
Ce2 O8 2.669(4) 2_655 ?
Ce2 O46 2.711(5) . ?
Ti1 O20 1.793(5) . ?
Ti1 O10 1.801(5) . ?
Ti1 O12 1.895(5) . ?
Ti1 O11 2.084(5) . ?
Ti1 O9 2.100(5) . ?
Ti1 O7 2.174(5) . ?
Ti1 Ti5 3.0727(18) . ?
Ti2 O24 1.786(5) . ?
Ti2 O34 1.793(5) . ?
Ti2 O22 1.897(4) . ?
Ti2 O35 2.087(5) . ?
Ti2 O26 2.097(5) . ?
Ti2 O21 2.180(5) . ?
Ti2 Ti6 3.0839(17) . ?
Ti3 O37 1.779(5) . ?
Ti3 O33 1.798(5) . ?
Ti3 O30 1.980(5) . ?
Ti3 O22 2.031(5) . ?
Ti3 O41 2.069(5) . ?
Ti3 O42 2.176(5) . ?
Ti3 Ti6 3.1162(18) . ?
Ti4 O17 1.770(5) . ?
Ti4 O13 1.783(5) . ?
Ti4 O14 1.982(5) . ?
Ti4 O12 2.057(5) . ?
Ti4 O16 2.067(5) . ?
Ti4 O15 2.168(5) . ?
Ti4 Ti5 3.1153(18) . ?
Ti5 O19 1.765(5) . ?
Ti5 O18 1.780(5) . ?
Ti5 O12 1.947(5) . ?
Ti5 O11 1.968(5) . ?
Ti5 O14 2.019(5) . ?
Ti6 O38 1.773(5) . ?
Ti6 O36 1.784(5) . ?
Ti6 O22 1.951(5) . ?
Ti6 O35 1.966(5) . ?
Ti6 O30 2.034(5) . ?
O1 C13 1.247(8) . ?
O2 C14 1.245(8) . ?
O3 N2 1.293(7) . ?
O4 C6 1.236(8) 2_655 ?
O5 C19 1.481(8) . ?
O6 C24 1.458(8) . ?
O7 C7 1.244(8) . ?
O8 C7 1.259(8) . ?
O9 C6 1.258(8) . ?
O10 C1 1.427(9) . ?
O11 C16 1.460(8) . ?
O13 C67 1.436(9) . ?
O14 C10 1.441(8) . ?
O15 C13 1.252(8) . ?
O16 C14 1.262(8) . ?
O17 C8 1.437(9) . ?
O18 C22 1.422(9) . ?
O19 C73 1.389(12) . ?
O20 C4 1.427(9) . ?
O21 C32 1.253(8) . ?
O23 C32 1.255(8) . ?
O24 C29 1.425(8) . ?
O25 C40 1.245(8) . ?
O26 C31 1.263(8) . ?
O27 N1 1.285(7) . ?
O28 N1 1.251(8) . ?
O29 C41 1.243(8) . ?
O30 C36 1.454(8) . ?
O31 C31 1.235(8) 2_556 ?
O32 C47 1.460(8) . ?
O33 C66 1.438(9) . ?
O34 C26 1.433(8) . ?
O35 C33 1.451(9) . ?
O36 C42 1.431(9) . ?
O37 C39 1.390(11) . ?
O38 C45 1.435(8) . ?
O39 C63 1.452(9) . ?
O40 C49 1.467(8) . ?
O41 C41 1.281(8) . ?
O42 C40 1.249(8) . ?
O43 N1 1.221(8) . ?
O44 C60 1.447(9) . ?
O46 N2 1.259(7) . ?
O47 N2 1.216(7) . ?
C1 C3 1.519(11) . ?
C1 C2 1.530(11) . ?
C4 C53 1.530(10) . ?
C4 C5 1.548(11) . ?
C6 C7 1.547(9) . ?
C8 C9 1.491(14) . ?
C8 C56 1.494(14) . ?
C10 C12 1.516(11) . ?
C10 C11 1.529(11) . ?
C13 C14 1.553(10) . ?
C15 C73 1.420(15) . ?
C16 C17 1.500(11) . ?
C16 C18 1.522(11) . ?
C19 C20 1.500(10) . ?
C19 C21 1.528(10) . ?
C22 C23 1.516(11) . ?
C22 C54 1.551(12) . ?
C24 C52 1.528(10) . ?
C24 C25 1.535(10) . ?
C26 C27 1.512(11) . ?
C26 C28 1.532(10) . ?
C29 C30 1.521(11) . ?
C29 C74 1.553(11) . ?
C31 C32 1.542(9) . ?
C33 C35 1.528(11) . ?
C33 C34 1.531(11) . ?
C36 C37 1.512(11) . ?
C36 C38 1.541(11) . ?
C39 C55 1.465(15) . ?
C39 C59 1.484(14) . ?
C40 C41 1.544(9) . ?
C42 C44 1.516(13) . ?
C42 C43 1.542(12) . ?
C45 C58 1.522(11) . ?
C45 C46 1.537(11) . ?
C47 C48 1.511(10) . ?
C47 C57 1.530(10) . ?
C49 C51 1.518(9) . ?
C49 C50 1.534(10) . ?
C60 C61 1.516(10) . ?
C60 C62 1.528(10) . ?
C63 C64 1.524(10) . ?
C63 C65 1.546(10) . ?
C66 C68 1.503(11) . ?
C66 C69 1.544(11) . ?
C67 C71 1.531(12) . ?
C67 C70 1.538(12) . ?
C72 C73 1.516(16) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O31 Ce1 O25 135.94(15) . . ?
O31 Ce1 O40 70.45(15) . . ?
O25 Ce1 O40 84.66(15) . . ?
O31 Ce1 O29 138.53(16) . . ?
O25 Ce1 O29 65.66(15) . . ?
O40 Ce1 O29 79.71(15) . . ?
O31 Ce1 O32 79.97(16) . . ?
O25 Ce1 O32 140.15(15) . . ?
O40 Ce1 O32 96.24(15) . . ?
O29 Ce1 O32 75.27(15) . . ?
O31 Ce1 O27 92.27(17) . . ?
O25 Ce1 O27 71.52(16) . . ?
O40 Ce1 O27 123.47(15) . . ?
O29 Ce1 O27 128.65(16) . . ?
O32 Ce1 O27 134.42(15) . . ?
O31 Ce1 O23 123.26(14) . . ?
O25 Ce1 O23 89.45(14) . . ?
O40 Ce1 O23 163.25(15) . . ?
O29 Ce1 O23 83.57(14) . . ?
O32 Ce1 O23 78.36(14) . . ?
O27 Ce1 O23 68.75(15) . . ?
O31 Ce1 O23 63.72(14) . 2_556 ?
O25 Ce1 O23 136.00(15) . 2_556 ?
O40 Ce1 O23 133.26(14) . 2_556 ?
O29 Ce1 O23 131.61(14) . 2_556 ?
O32 Ce1 O23 67.89(14) . 2_556 ?
O27 Ce1 O23 68.47(15) . 2_556 ?
O23 Ce1 O23 59.56(17) . 2_556 ?
O31 Ce1 O28 72.24(15) . . ?
O25 Ce1 O28 66.44(15) . . ?
O40 Ce1 O28 75.30(14) . . ?
O29 Ce1 O28 127.32(14) . . ?
O32 Ce1 O28 152.20(15) . . ?
O27 Ce1 O28 48.28(14) . . ?
O23 Ce1 O28 116.52(14) . . ?
O23 Ce1 O28 98.36(14) 2_556 . ?
O4 Ce2 O1 136.90(16) . . ?
O4 Ce2 O6 70.84(15) . . ?
O1 Ce2 O6 84.60(15) . . ?
O4 Ce2 O2 137.16(15) . . ?
O1 Ce2 O2 66.12(15) . . ?
O6 Ce2 O2 78.83(15) . . ?
O4 Ce2 O5 79.48(16) . . ?
O1 Ce2 O5 139.93(16) . . ?
O6 Ce2 O5 97.03(15) . . ?
O2 Ce2 O5 74.91(15) . . ?
O4 Ce2 O3 91.80(17) . . ?
O1 Ce2 O3 72.20(16) . . ?
O6 Ce2 O3 122.94(15) . . ?
O2 Ce2 O3 130.53(16) . . ?
O5 Ce2 O3 133.78(15) . . ?
O4 Ce2 O8 125.27(14) . . ?
O1 Ce2 O8 86.41(15) . . ?
O6 Ce2 O8 162.06(15) . . ?
O2 Ce2 O8 83.34(14) . . ?
O5 Ce2 O8 80.08(15) . . ?
O3 Ce2 O8 68.34(15) . . ?
O4 Ce2 O8 64.11(14) . 2_655 ?
O1 Ce2 O8 135.39(14) . 2_655 ?
O6 Ce2 O8 134.18(14) . 2_655 ?
O2 Ce2 O8 131.43(14) . 2_655 ?
O5 Ce2 O8 67.59(14) . 2_655 ?
O3 Ce2 O8 67.82(15) . 2_655 ?
O8 Ce2 O8 61.16(17) . 2_655 ?
O4 Ce2 O46 72.00(15) . . ?
O1 Ce2 O46 67.54(15) . . ?
O6 Ce2 O46 74.73(14) . . ?
O2 Ce2 O46 128.05(14) . . ?
O5 Ce2 O46 151.47(15) . . ?
O3 Ce2 O46 48.32(14) . . ?
O8 Ce2 O46 115.80(14) . . ?
O8 Ce2 O46 98.26(14) 2_655 . ?
O20 Ti1 O10 97.7(2) . . ?
O20 Ti1 O12 101.3(2) . . ?
O10 Ti1 O12 106.4(2) . . ?
O20 Ti1 O11 169.9(2) . . ?
O10 Ti1 O11 92.4(2) . . ?
O12 Ti1 O11 75.62(19) . . ?
O20 Ti1 O9 91.6(2) . . ?
O10 Ti1 O9 90.8(2) . . ?
O12 Ti1 O9 156.7(2) . . ?
O11 Ti1 O9 88.32(19) . . ?
O20 Ti1 O7 85.1(2) . . ?
O10 Ti1 O7 164.9(2) . . ?
O12 Ti1 O7 87.43(18) . . ?
O11 Ti1 O7 85.17(18) . . ?
O9 Ti1 O7 74.32(17) . . ?
O20 Ti1 Ti5 138.71(16) . . ?
O10 Ti1 Ti5 94.94(16) . . ?
O12 Ti1 Ti5 37.47(14) . . ?
O11 Ti1 Ti5 39.30(13) . . ?
O9 Ti1 Ti5 127.41(15) . . ?
O7 Ti1 Ti5 92.54(13) . . ?
O24 Ti2 O34 97.4(2) . . ?
O24 Ti2 O22 104.3(2) . . ?
O34 Ti2 O22 101.5(2) . . ?
O24 Ti2 O35 93.0(2) . . ?
O34 Ti2 O35 169.6(2) . . ?
O22 Ti2 O35 75.13(19) . . ?
O24 Ti2 O26 92.1(2) . . ?
O34 Ti2 O26 92.9(2) . . ?
O22 Ti2 O26 156.5(2) . . ?
O35 Ti2 O26 87.43(18) . . ?
O24 Ti2 O21 166.5(2) . . ?
O34 Ti2 O21 86.0(2) . . ?
O22 Ti2 O21 87.72(18) . . ?
O35 Ti2 O21 84.03(19) . . ?
O26 Ti2 O21 74.71(17) . . ?
O24 Ti2 Ti6 93.77(15) . . ?
O34 Ti2 Ti6 138.77(16) . . ?
O22 Ti2 Ti6 37.33(14) . . ?
O35 Ti2 Ti6 39.01(13) . . ?
O26 Ti2 Ti6 126.33(14) . . ?
O21 Ti2 Ti6 92.17(13) . . ?
O37 Ti3 O33 98.5(2) . . ?
O37 Ti3 O30 101.4(2) . . ?
O33 Ti3 O30 104.6(2) . . ?
O37 Ti3 O22 170.6(2) . . ?
O33 Ti3 O22 90.7(2) . . ?
O30 Ti3 O22 74.79(19) . . ?
O37 Ti3 O41 92.5(2) . . ?
O33 Ti3 O41 95.8(2) . . ?
O30 Ti3 O41 153.2(2) . . ?
O22 Ti3 O41 87.88(18) . . ?
O37 Ti3 O42 90.3(2) . . ?
O33 Ti3 O42 168.3(2) . . ?
O30 Ti3 O42 81.03(19) . . ?
O22 Ti3 O42 80.72(18) . . ?
O41 Ti3 O42 76.01(18) . . ?
O37 Ti3 Ti6 135.81(17) . . ?
O33 Ti3 Ti6 109.67(17) . . ?
O30 Ti3 Ti6 39.69(14) . . ?
O22 Ti3 Ti6 37.59(13) . . ?
O41 Ti3 Ti6 116.75(14) . . ?
O42 Ti3 Ti6 67.94(13) . . ?
O17 Ti4 O13 98.3(2) . . ?
O17 Ti4 O14 98.6(2) . . ?
O13 Ti4 O14 104.6(2) . . ?
O17 Ti4 O12 170.2(2) . . ?
O13 Ti4 O12 90.2(2) . . ?
O14 Ti4 O12 74.52(19) . . ?
O17 Ti4 O16 95.0(2) . . ?
O13 Ti4 O16 94.1(2) . . ?
O14 Ti4 O16 154.9(2) . . ?
O12 Ti4 O16 89.09(18) . . ?
O17 Ti4 O15 91.2(2) . . ?
O13 Ti4 O15 167.1(2) . . ?
O14 Ti4 O15 82.36(19) . . ?
O12 Ti4 O15 81.11(18) . . ?
O16 Ti4 O15 76.28(18) . . ?
O17 Ti4 Ti5 133.56(19) . . ?
O13 Ti4 Ti5 109.24(17) . . ?
O14 Ti4 Ti5 39.30(13) . . ?
O12 Ti4 Ti5 37.66(13) . . ?
O16 Ti4 Ti5 118.61(13) . . ?
O15 Ti4 Ti5 69.19(13) . . ?
O19 Ti5 O18 108.0(3) . . ?
O19 Ti5 O12 114.6(2) . . ?
O18 Ti5 O12 137.2(2) . . ?
O19 Ti5 O11 101.6(2) . . ?
O18 Ti5 O11 98.1(2) . . ?
O12 Ti5 O11 77.24(19) . . ?
O19 Ti5 O14 98.7(2) . . ?
O18 Ti5 O14 94.4(2) . . ?
O12 Ti5 O14 76.13(19) . . ?
O11 Ti5 O14 151.4(2) . . ?
O19 Ti5 Ti1 106.54(18) . . ?
O18 Ti5 Ti1 131.77(17) . . ?
O12 Ti5 Ti1 36.30(13) . . ?
O11 Ti5 Ti1 42.12(14) . . ?
O14 Ti5 Ti1 112.41(15) . . ?
O19 Ti5 Ti4 121.32(19) . . ?
O18 Ti5 Ti4 111.91(17) . . ?
O12 Ti5 Ti4 40.20(13) . . ?
O11 Ti5 Ti4 113.04(14) . . ?
O14 Ti5 Ti4 38.44(14) . . ?
Ti1 Ti5 Ti4 75.78(4) . . ?
O38 Ti6 O36 104.6(2) . . ?
O38 Ti6 O22 137.7(2) . . ?
O36 Ti6 O22 117.6(2) . . ?
O38 Ti6 O35 99.5(2) . . ?
O36 Ti6 O35 100.4(2) . . ?
O22 Ti6 O35 76.82(19) . . ?
O38 Ti6 O30 94.8(2) . . ?
O36 Ti6 O30 100.6(2) . . ?
O22 Ti6 O30 75.35(19) . . ?
O35 Ti6 O30 150.7(2) . . ?
O38 Ti6 Ti2 133.09(17) . . ?
O36 Ti6 Ti2 107.62(16) . . ?
O22 Ti6 Ti2 36.14(13) . . ?
O35 Ti6 Ti2 41.93(14) . . ?
O30 Ti6 Ti2 111.43(14) . . ?
O38 Ti6 Ti3 112.57(17) . . ?
O36 Ti6 Ti3 124.23(17) . . ?
O22 Ti6 Ti3 39.43(13) . . ?
O35 Ti6 Ti3 112.23(14) . . ?
O30 Ti6 Ti3 38.44(14) . . ?
Ti2 Ti6 Ti3 74.96(4) . . ?
C13 O1 Ce2 119.7(4) . . ?
C14 O2 Ce2 117.7(4) . . ?
N2 O3 Ce2 102.1(4) . . ?
C6 O4 Ce2 123.8(4) 2_655 . ?
C19 O5 Ce2 138.0(4) . . ?
C24 O6 Ce2 128.1(4) . . ?
C7 O7 Ti1 116.3(4) . . ?
C7 O8 Ce2 125.4(4) . . ?
C7 O8 Ce2 115.6(4) . 2_655 ?
Ce2 O8 Ce2 118.84(17) . 2_655 ?
C6 O9 Ti1 119.0(4) . . ?
C1 O10 Ti1 131.3(5) . . ?
C16 O11 Ti5 120.4(4) . . ?
C16 O11 Ti1 137.8(4) . . ?
Ti5 O11 Ti1 98.6(2) . . ?
Ti1 O12 Ti5 106.2(2) . . ?
Ti1 O12 Ti4 148.2(3) . . ?
Ti5 O12 Ti4 102.1(2) . . ?
C67 O13 Ti4 140.1(5) . . ?
C10 O14 Ti4 134.1(4) . . ?
C10 O14 Ti5 123.4(4) . . ?
Ti4 O14 Ti5 102.3(2) . . ?
C13 O15 Ti4 114.9(4) . . ?
C14 O16 Ti4 118.7(4) . . ?
C8 O17 Ti4 152.1(6) . . ?
C22 O18 Ti5 148.0(5) . . ?
C73 O19 Ti5 162.6(7) . . ?
C4 O20 Ti1 150.0(5) . . ?
C32 O21 Ti2 115.6(4) . . ?
Ti2 O22 Ti6 106.5(2) . . ?
Ti2 O22 Ti3 147.6(3) . . ?
Ti6 O22 Ti3 103.0(2) . . ?
C32 O23 Ce1 124.5(4) . . ?
C32 O23 Ce1 114.8(4) . 2_556 ?
Ce1 O23 Ce1 120.45(17) . 2_556 ?
C29 O24 Ti2 139.1(5) . . ?
C40 O25 Ce1 119.9(4) . . ?
C31 O26 Ti2 118.8(4) . . ?
N1 O27 Ce1 101.7(4) . . ?
N1 O28 Ce1 93.1(4) . . ?
C41 O29 Ce1 117.2(4) . . ?
C36 O30 Ti3 134.2(4) . . ?
C36 O30 Ti6 123.6(4) . . ?
Ti3 O30 Ti6 101.9(2) . . ?
C31 O31 Ce1 124.6(4) 2_556 . ?
C47 O32 Ce1 138.7(4) . . ?
C66 O33 Ti3 137.2(4) . . ?
C26 O34 Ti2 149.9(4) . . ?
C33 O35 Ti6 121.0(4) . . ?
C33 O35 Ti2 135.9(4) . . ?
Ti6 O35 Ti2 99.1(2) . . ?
C42 O36 Ti6 136.8(5) . . ?
C39 O37 Ti3 158.6(7) . . ?
C45 O38 Ti6 148.9(5) . . ?
C49 O40 Ce1 128.3(4) . . ?
C41 O41 Ti3 118.2(4) . . ?
C40 O42 Ti3 115.6(4) . . ?
N2 O46 Ce2 94.1(4) . . ?
O43 N1 O28 123.0(6) . . ?
O43 N1 O27 121.0(6) . . ?
O28 N1 O27 116.0(6) . . ?
O47 N2 O46 124.4(6) . . ?
O47 N2 O3 120.8(6) . . ?
O46 N2 O3 114.8(5) . . ?
O10 C1 C3 109.6(6) . . ?
O10 C1 C2 108.1(7) . . ?
C3 C1 C2 113.4(7) . . ?
O20 C4 C53 109.0(6) . . ?
O20 C4 C5 107.7(6) . . ?
C53 C4 C5 111.5(6) . . ?
O4 C6 O9 127.3(6) 2_655 . ?
O4 C6 C7 118.5(6) 2_655 . ?
O9 C6 C7 114.2(6) . . ?
O7 C7 O8 127.6(6) . . ?
O7 C7 C6 114.7(6) . . ?
O8 C7 C6 117.7(6) . . ?
O17 C8 C9 109.0(8) . . ?
O17 C8 C56 109.7(7) . . ?
C9 C8 C56 115.8(10) . . ?
O14 C10 C12 109.2(6) . . ?
O14 C10 C11 111.1(6) . . ?
C12 C10 C11 113.0(7) . . ?
O1 C13 O15 127.4(7) . . ?
O1 C13 C14 117.0(6) . . ?
O15 C13 C14 115.6(6) . . ?
O2 C14 O16 127.7(7) . . ?
O2 C14 C13 117.8(6) . . ?
O16 C14 C13 114.5(6) . . ?
O11 C16 C17 110.1(6) . . ?
O11 C16 C18 110.4(6) . . ?
C17 C16 C18 112.4(7) . . ?
O5 C19 C20 107.1(5) . . ?
O5 C19 C21 109.5(6) . . ?
C20 C19 C21 113.8(6) . . ?
O18 C22 C23 109.5(7) . . ?
O18 C22 C54 108.4(6) . . ?
C23 C22 C54 112.6(7) . . ?
O6 C24 C52 109.4(6) . . ?
O6 C24 C25 109.0(6) . . ?
C52 C24 C25 112.6(6) . . ?
O34 C26 C27 108.6(6) . . ?
O34 C26 C28 108.5(6) . . ?
C27 C26 C28 112.8(7) . . ?
O24 C29 C30 107.4(6) . . ?
O24 C29 C74 109.3(6) . . ?
C30 C29 C74 111.7(7) . . ?
O31 C31 O26 127.3(6) 2_556 . ?
O31 C31 C32 118.4(6) 2_556 . ?
O26 C31 C32 114.3(6) . . ?
O21 C32 O23 126.6(6) . . ?
O21 C32 C31 115.2(6) . . ?
O23 C32 C31 118.2(6) . . ?
O35 C33 C35 110.5(6) . . ?
O35 C33 C34 110.3(6) . . ?
C35 C33 C34 112.4(7) . . ?
O30 C36 C37 108.6(6) . . ?
O30 C36 C38 109.8(6) . . ?
C37 C36 C38 111.7(7) . . ?
O37 C39 C55 114.0(10) . . ?
O37 C39 C59 112.7(8) . . ?
C55 C39 C59 119.5(10) . . ?
O25 C40 O42 128.1(6) . . ?
O25 C40 C41 116.8(6) . . ?
O42 C40 C41 115.1(6) . . ?
O29 C41 O41 126.7(6) . . ?
O29 C41 C40 118.3(6) . . ?
O41 C41 C40 115.0(6) . . ?
O36 C42 C44 108.3(7) . . ?
O36 C42 C43 109.1(6) . . ?
C44 C42 C43 111.2(8) . . ?
O38 C45 C58 108.2(6) . . ?
O38 C45 C46 107.4(6) . . ?
C58 C45 C46 112.2(7) . . ?
O32 C47 C48 107.5(5) . . ?
O32 C47 C57 109.4(6) . . ?
C48 C47 C57 113.5(6) . . ?
O40 C49 C51 109.9(6) . . ?
O40 C49 C50 108.4(6) . . ?
C51 C49 C50 112.4(6) . . ?
O44 C60 C61 110.0(6) . . ?
O44 C60 C62 111.1(6) . . ?
C61 C60 C62 113.3(6) . . ?
O39 C63 C64 111.0(6) . . ?
O39 C63 C65 108.9(6) . . ?
C64 C63 C65 113.3(6) . . ?
O33 C66 C68 109.0(6) . . ?
O33 C66 C69 107.2(6) . . ?
C68 C66 C69 112.8(7) . . ?
O13 C67 C71 108.3(6) . . ?
O13 C67 C70 108.0(7) . . ?
C71 C67 C70 112.4(7) . . ?
O19 C73 C15 114.8(10) . . ?
O19 C73 C72 110.5(10) . . ?
C15 C73 C72 119.7(12) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O20 Ti1 O10 C1 -31.7(6) . . . . ?
O12 Ti1 O10 C1 -135.9(6) . . . . ?
O11 Ti1 O10 C1 148.4(6) . . . . ?
O9 Ti1 O10 C1 60.1(6) . . . . ?
O7 Ti1 O10 C1 68.2(11) . . . . ?
Ti5 Ti1 O10 C1 -172.3(6) . . . . ?
O20 Ti1 O12 Ti5 -178.0(2) . . . . ?
O10 Ti1 O12 Ti5 -76.4(3) . . . . ?
O11 Ti1 O12 Ti5 11.9(2) . . . . ?
O9 Ti1 O12 Ti5 59.6(6) . . . . ?
O7 Ti1 O12 Ti5 97.6(2) . . . . ?
O20 Ti1 O12 Ti4 30.0(5) . . . . ?
O10 Ti1 O12 Ti4 131.6(5) . . . . ?
O11 Ti1 O12 Ti4 -140.2(5) . . . . ?
O9 Ti1 O12 Ti4 -92.4(7) . . . . ?
O7 Ti1 O12 Ti4 -54.5(5) . . . . ?
Ti5 Ti1 O12 Ti4 -152.1(6) . . . . ?
O17 Ti4 O13 C67 -175.8(7) . . . . ?
O14 Ti4 O13 C67 83.0(8) . . . . ?
O12 Ti4 O13 C67 9.0(8) . . . . ?
O16 Ti4 O13 C67 -80.1(8) . . . . ?
O15 Ti4 O13 C67 -38.5(14) . . . . ?
Ti5 Ti4 O13 C67 42.1(8) . . . . ?
O13 Ti4 O17 C8 14.1(12) . . . . ?
O14 Ti4 O17 C8 120.4(12) . . . . ?
O16 Ti4 O17 C8 -80.8(12) . . . . ?
O15 Ti4 O17 C8 -157.1(12) . . . . ?
Ti5 Ti4 O17 C8 140.9(11) . . . . ?
O19 Ti5 O18 C22 159.1(9) . . . . ?
O12 Ti5 O18 C22 -15.9(10) . . . . ?
O11 Ti5 O18 C22 -95.9(9) . . . . ?
O14 Ti5 O18 C22 58.4(9) . . . . ?
Ti1 Ti5 O18 C22 -67.2(9) . . . . ?
Ti4 Ti5 O18 C22 23.1(9) . . . . ?
O18 Ti5 O19 C73 18(2) . . . . ?
O12 Ti5 O19 C73 -166(2) . . . . ?
O11 Ti5 O19 C73 -85(2) . . . . ?
O14 Ti5 O19 C73 116(2) . . . . ?
Ti1 Ti5 O19 C73 -128(2) . . . . ?
Ti4 Ti5 O19 C73 149(2) . . . . ?
O10 Ti1 O20 C4 151.7(9) . . . . ?
O12 Ti1 O20 C4 -99.8(9) . . . . ?
O11 Ti1 O20 C4 -28.8(17) . . . . ?
O9 Ti1 O20 C4 60.7(9) . . . . ?
O7 Ti1 O20 C4 -13.4(9) . . . . ?
Ti5 Ti1 O20 C4 -101.7(8) . . . . ?
O24 Ti2 O22 Ti6 77.2(3) . . . . ?
O34 Ti2 O22 Ti6 178.0(2) . . . . ?
O35 Ti2 O22 Ti6 -12.2(2) . . . . ?
O26 Ti2 O22 Ti6 -55.5(6) . . . . ?
O21 Ti2 O22 Ti6 -96.6(2) . . . . ?
O24 Ti2 O22 Ti3 -127.9(5) . . . . ?
O34 Ti2 O22 Ti3 -27.1(5) . . . . ?
O35 Ti2 O22 Ti3 142.7(5) . . . . ?
O26 Ti2 O22 Ti3 99.4(6) . . . . ?
O21 Ti2 O22 Ti3 58.3(5) . . . . ?
Ti6 Ti2 O22 Ti3 154.9(6) . . . . ?
O34 Ti2 O24 C29 20.1(7) . . . . ?
O22 Ti2 O24 C29 123.9(7) . . . . ?
O35 Ti2 O24 C29 -160.6(7) . . . . ?
O26 Ti2 O24 C29 -73.1(7) . . . . ?
O21 Ti2 O24 C29 -83.7(11) . . . . ?
Ti6 Ti2 O24 C29 160.3(7) . . . . ?
O37 Ti3 O33 C66 173.0(7) . . . . ?
O30 Ti3 O33 C66 -82.9(7) . . . . ?
O22 Ti3 O33 C66 -8.4(7) . . . . ?
O41 Ti3 O33 C66 79.6(7) . . . . ?
O42 Ti3 O33 C66 34.5(15) . . . . ?
Ti6 Ti3 O33 C66 -41.6(7) . . . . ?
O24 Ti2 O34 C26 -156.6(8) . . . . ?
O22 Ti2 O34 C26 97.1(9) . . . . ?
O35 Ti2 O34 C26 27.2(17) . . . . ?
O26 Ti2 O34 C26 -64.1(9) . . . . ?
O21 Ti2 O34 C26 10.3(8) . . . . ?
Ti6 Ti2 O34 C26 99.0(8) . . . . ?
O38 Ti6 O36 C42 -1.0(7) . . . . ?
O22 Ti6 O36 C42 -177.8(6) . . . . ?
O35 Ti6 O36 C42 101.8(7) . . . . ?
O30 Ti6 O36 C42 -98.9(7) . . . . ?
Ti2 Ti6 O36 C42 144.4(6) . . . . ?
Ti3 Ti6 O36 C42 -132.1(6) . . . . ?
O33 Ti3 O37 C39 -94.5(18) . . . . ?
O30 Ti3 O37 C39 158.6(18) . . . . ?
O41 Ti3 O37 C39 1.7(18) . . . . ?
O42 Ti3 O37 C39 77.7(18) . . . . ?
Ti6 Ti3 O37 C39 135.5(17) . . . . ?
O36 Ti6 O38 C45 -157.6(9) . . . . ?
O22 Ti6 O38 C45 18.1(10) . . . . ?
O35 Ti6 O38 C45 98.9(9) . . . . ?
O30 Ti6 O38 C45 -55.4(9) . . . . ?
Ti2 Ti6 O38 C45 70.1(9) . . . . ?
Ti3 Ti6 O38 C45 -20.1(9) . . . . ?
Ce1 O28 N1 O43 -171.8(6) . . . . ?
Ce1 O28 N1 O27 8.9(6) . . . . ?
Ce1 O27 N1 O43 170.9(5) . . . . ?
Ce1 O27 N1 O28 -9.9(6) . . . . ?
Ce2 O46 N2 O47 171.6(6) . . . . ?
Ce2 O46 N2 O3 -8.0(6) . . . . ?
Ce2 O3 N2 O47 -170.9(5) . . . . ?
Ce2 O3 N2 O46 8.8(6) . . . . ?
Ti1 O10 C1 C3 93.5(8) . . . . ?
Ti1 O10 C1 C2 -142.4(6) . . . . ?
Ti1 O20 C4 C53 -96.8(9) . . . . ?
Ti1 O20 C4 C5 142.1(7) . . . . ?
Ti1 O9 C6 O4 174.3(6) . . . 2_655 ?
Ti1 O9 C6 C7 -6.0(8) . . . . ?
Ti1 O7 C7 O8 -167.2(5) . . . . ?
Ti1 O7 C7 C6 11.7(7) . . . . ?
Ce2 O8 C7 O7 0.5(10) . . . . ?
Ce2 O8 C7 O7 -175.4(5) 2_655 . . . ?
Ce2 O8 C7 C6 -178.4(4) . . . . ?
Ce2 O8 C7 C6 5.7(7) 2_655 . . . ?
O4 C6 C7 O7 175.5(6) 2_655 . . . ?
O9 C6 C7 O7 -4.2(9) . . . . ?
O4 C6 C7 O8 -5.4(9) 2_655 . . . ?
O9 C6 C7 O8 174.9(6) . . . . ?
Ti4 O17 C8 C9 153.5(10) . . . . ?
Ti4 O17 C8 C56 25.7(17) . . . . ?
Ti4 O14 C10 C12 -64.9(8) . . . . ?
Ti5 O14 C10 C12 121.4(6) . . . . ?
Ti4 O14 C10 C11 60.3(9) . . . . ?
Ti5 O14 C10 C11 -113.4(6) . . . . ?
Ce2 O1 C13 O15 -171.3(5) . . . . ?
Ce2 O1 C13 C14 8.9(7) . . . . ?
Ti4 O15 C13 O1 178.8(5) . . . . ?
Ti4 O15 C13 C14 -1.5(7) . . . . ?
Ce2 O2 C14 O16 170.3(5) . . . . ?
Ce2 O2 C14 C13 -10.9(7) . . . . ?
Ti4 O16 C14 O2 179.2(5) . . . . ?
Ti4 O16 C14 C13 0.4(7) . . . . ?
O1 C13 C14 O2 1.6(9) . . . . ?
O15 C13 C14 O2 -178.2(6) . . . . ?
O1 C13 C14 O16 -179.4(6) . . . . ?
O15 C13 C14 O16 0.8(8) . . . . ?
Ti5 O11 C16 C17 -105.5(6) . . . . ?
Ti1 O11 C16 C17 48.9(9) . . . . ?
Ti5 O11 C16 C18 129.8(5) . . . . ?
Ti1 O11 C16 C18 -75.7(8) . . . . ?
Ce2 O5 C19 C20 -26.2(9) . . . . ?
Ce2 O5 C19 C21 97.6(7) . . . . ?
Ti5 O18 C22 C23 -150.6(7) . . . . ?
Ti5 O18 C22 C54 86.2(10) . . . . ?
Ce2 O6 C24 C52 108.9(6) . . . . ?
Ce2 O6 C24 C25 -127.6(5) . . . . ?
Ti2 O34 C26 C27 -141.6(7) . . . . ?
Ti2 O34 C26 C28 95.6(9) . . . . ?
Ti2 O24 C29 C30 -171.8(6) . . . . ?
Ti2 O24 C29 C74 66.9(10) . . . . ?
Ti2 O26 C31 O31 -174.4(5) . . . 2_556 ?
Ti2 O26 C31 C32 6.9(7) . . . . ?
Ti2 O21 C32 O23 168.9(5) . . . . ?
Ti2 O21 C32 C31 -10.5(7) . . . . ?
Ce1 O23 C32 O21 0.5(9) . . . . ?
Ce1 O23 C32 O21 174.5(5) 2_556 . . . ?
Ce1 O23 C32 C31 179.9(4) . . . . ?
Ce1 O23 C32 C31 -6.1(7) 2_556 . . . ?
O31 C31 C32 O21 -176.0(6) 2_556 . . . ?
O26 C31 C32 O21 2.8(8) . . . . ?
O31 C31 C32 O23 4.5(9) 2_556 . . . ?
O26 C31 C32 O23 -176.6(6) . . . . ?
Ti6 O35 C33 C35 111.4(6) . . . . ?
Ti2 O35 C33 C35 -40.6(9) . . . . ?
Ti6 O35 C33 C34 -123.6(5) . . . . ?
Ti2 O35 C33 C34 84.4(8) . . . . ?
Ti3 O30 C36 C37 63.5(8) . . . . ?
Ti6 O30 C36 C37 -125.0(6) . . . . ?
Ti3 O30 C36 C38 -58.8(9) . . . . ?
Ti6 O30 C36 C38 112.7(6) . . . . ?
Ti3 O37 C39 C55 -101.4(16) . . . . ?
Ti3 O37 C39 C59 39(3) . . . . ?
Ce1 O25 C40 O42 170.3(5) . . . . ?
Ce1 O25 C40 C41 -11.6(7) . . . . ?
Ti3 O42 C40 O25 -179.0(5) . . . . ?
Ti3 O42 C40 C41 2.8(7) . . . . ?
Ce1 O29 C41 O41 -167.4(5) . . . . ?
Ce1 O29 C41 C40 11.9(7) . . . . ?
Ti3 O41 C41 O29 -179.3(5) . . . . ?
Ti3 O41 C41 C40 1.4(7) . . . . ?
O25 C40 C41 O29 -0.6(9) . . . . ?
O42 C40 C41 O29 177.8(6) . . . . ?
O25 C40 C41 O41 178.8(6) . . . . ?
O42 C40 C41 O41 -2.9(8) . . . . ?
Ti6 O36 C42 C44 123.4(8) . . . . ?
Ti6 O36 C42 C43 -115.4(7) . . . . ?
Ti6 O38 C45 C58 145.5(8) . . . . ?
Ti6 O38 C45 C46 -93.3(10) . . . . ?
Ce1 O32 C47 C48 22.5(9) . . . . ?
Ce1 O32 C47 C57 -101.1(7) . . . . ?
Ce1 O40 C49 C51 124.4(5) . . . . ?
Ce1 O40 C49 C50 -112.4(5) . . . . ?
Ti3 O33 C66 C68 84.4(8) . . . . ?
Ti3 O33 C66 C69 -153.2(6) . . . . ?
Ti4 O13 C67 C71 150.2(6) . . . . ?
Ti4 O13 C67 C70 -87.8(8) . . . . ?
Ti5 O19 C73 C15 -64(3) . . . . ?
Ti5 O19 C73 C72 157.4(16) . . . . ?

_refine_diff_density_max         1.508
_refine_diff_density_min         -0.868
_refine_diff_density_rms         0.174
